Investigation of interactions in twodimensional electron ... · Investigation of interactions in...

Upload
duongnguyet 
Category
Documents

view
218 
download
0
Embed Size (px)
Transcript of Investigation of interactions in twodimensional electron ... · Investigation of interactions in...
Investigation of interactions
in twodimensional electron gases
with angular resolved photoemission spectroscopy
Carola Straÿer
PhD Thesis
Max Planck Institute for Solid State Research in Stuttgart
Ecole Polytechnique Fédérale de Lausanne
March 25, 2015
ii
Abstract
In this thesis, angular resolved photoemission spectroscopy (ARPES) is used to study
the electronic structure of dierent twodimensional electron systems (2DES). This tech
nique is very surface sensitive and the most direct method to probe the surface band
structure of a system. In addition to the band dispersion also signatures from interac
tions can be detected with ARPES. A careful analysis of peak position and linewidth gives
access to the complex selfenergy Σ, which describes the energy renormalization and the
lifetime of the electrons due to manybody interactions. By using circularly polarized light
it is possible to excite electrons selectively and to extract additional information about the
electronic states in the surface.
2DESs exist typically either at interfaces or at surfaces. We put our focus on the
surface states of topological insulators and investigate Bi2Te2Se and TiTe1.5Se0.5. The rst
is known to be a topological insulator with the Fermi energy located in the bulk band gap.
A timedependent doping behavior is observed and we show that the Coulomb interaction
in this material is strongly dependent on the charge carrier density and not negligible for
very low concentrations. TiTe1.5Se0.5 was predicted to be a topological insulator. We are
able to present the surface band structure, but due to the fact that ARPES can only probe
the occupied states it is impossible to see the predicted topological surface states.
The third system under investigation is a monolayer of epitaxial graphene on SiC(0001)
decorated by small amounts of Tl adatoms. ARPES measurements at very low temperature
and very low impurity concentrations show that Tl adatoms not only give rise to electron
doping but have also a large eect on the quasiparticle scattering rate. The adatoms
introduce disorder and act on the graphene electronic structure both as Coulomb long
range scatterers as well as shortrange scatterers with a δlike potential. We show that
also for charged impurities shortrange scattering can play an important role and is not
always negligible. By modeling the selfenergy for long and shortrange scattering, we
are able to extract a strong shortrange scattering potential δ = −3.2 ± 1 eV. A detailed
understanding of the underlying scattering mechanisms in graphene is very important for
the development of novel impuritygraphenebased electronics.
ARPES experiments are also performed on the surface alloys on Ag(111). For these
measurements, we use circularly polarized light and take advantage of the fact that the
interaction between light and matter changes for dierent polarizations. Surface alloys on
Ag(111) are formed by depositing 1/3 of a monolayer of bismuth or antimony on the clean
Ag(111) surface, where every third Ag atom is replaced by such an alloy atom. These sys
iii
tems are known for their Rashba type spin splitting and the resulting chiral spin structure
in the twodimensional (2D) band structure. We show that circular dichroism (CD) in the
angular distribution of the photoelectrons depends strongly on the experimental setup and
the energy of the photons. Only under special circumstances it is possible to use CD to
access the orbital angular momentum and in systems with high spinorbit coupling
maybe even the spin texture of the surface. Because of the nal state eects, interpretation
of CD data is quite complicated and has to be done very cautiously.
Keywords: ARPEStwodimensional electron systemsgraphenetopological insulatorsurface alloysscattering mechanismsCoulomb interactionorbital angular momentumspintronics
iv
Zusammenfassung
In der vorliegenden Arbeit wird die elektronische Struktur von verschiedenen zwei
dimensionalen (2D) Elektronensystemen mit winkelaufgelöster Photoemission untersucht.
Diese Technik ist sehr oberächensensitiv und ermöglicht es direkt die Oberächenband
struktur eines Materials zu messen. Nicht nur die Dispersion der Bänder sondern auch
elektronische Wechselwirkungen können gemessen werden. Durch sorgfältige Bestimmung
von Peakpositionen und breiten kann man die komplexe Selbstenergie Σ berechnen, die den
Einuss der Wechselwirkung von Elektronen mit anderen Teilchen auf die Bindungsener
gie und die Lebensdauer der Elektronen beschreibt. Wählt man die zirkular polarisiertes
Licht, ist es sogar möglich gezielt Elektronen anzuregen und zusätzliche Information über
die elektronischen Zustände an der Oberäche zu gewinnen.
2D Elektronensysteme existieren typischerweise entweder an Grenzächen oder an Ober
ächen. Wir legen unseren Fokus auf die Oberächenzustände von topologischen Isolatoren
und untersuchen Bi2Te2Se und TiTe1.5Se0.5. Das erste Material ist bekannt als toloplogi
scher Isolator, bei dem die Fermienergie in der Bulkenergielücke liegt. Wir beobachten ein
zeitabhängiges Dopingverhalten und wir können zeigen, dass die CoulombWechselwirkung
in diesem Material stark von der Ladungsträgerdichte abhängt und für kleine Ladungsträ
gerdichten nicht vernachlässigbar ist. TiTe1.5Se0.5 wurde als neuer topologischer Isolator
vorgeschlagen. Wir präsentieren die Oberächenbandstruktur, allerdings ist es nicht mög
lich die topologischen Oberächenzustände zu beobachten, da mit Photoemission unbe
setzte Elektronenzustände nicht gemessen werden können.
Das dritte System, das wir im Folgenden untersuchen werden, ist eine Monolage von
epitaktischem Graphen auf SiC(0001) bedeckt mit einer kleinen Menge von Thalliumada
tomen. Photoemissionsmessungen bei sehr tiefen Temperaturen und sehr kleinen Konzen
trationen zeigen, dass Thalliumatome nicht nur Elektronen abgeben sondern auch einen
groÿen Einuss auf die Streurate der Elektronen haben. Die Adatome bringen Unordnung in
das System und wirken auf die elektronischen Struktur von Graphen sowohl als Coulomb
Streuer als auch als kurzreichweitige Streuzentren mit einem δförmigen Streupotential.
Wir zeigen, dass auch für geladene Streuzentren kurzreichweitige Streumechanismen eine
wichtige Rolle spielen können und nicht immer vernachlässigbar sind. Durch Modellie
rung der Selbstenergie für lang und kurzreichweitige Streuung sind wir in der Lage für
das δPotential einen Wert von δ = −3.2 ± 1 eV zu extrahieren. Die zugrunde liegenden
Streumechanismen in Graphen zu verstehen ist ein sehr wichtiges Ziel im Hinblick auf die
Entwicklung von elektronischen Bauteilen, die auf mit Störstellen dekoriertem Graphen
v
basieren.
Auÿerdem zeigen wir Ergebnisse von Experimenten an Oberächenlegierungen auf
Ag(111). Für diese Messungen verwenden wir zirkular polarisiertes Licht und nutzen den
Vorteil, dass sich die Wechselwirkung zwischen Licht und Materie für verschiedene Polari
sationen ändert. Oberächenlegierungen auf Ag(111) bilden sich, wenn man 1/3 Monolage
Wismuth oder Antimon auf eine saubere Silberoberäche aufdampft. Dabei wird jedes drit
te Silberatom von einem solchen Legierungsatom ersetzt. Diese Legierungen sind bekannt
für die Rashbaartige Spinaufspaltung und die daraus resultierende chirale SpinStruktur
in der 2D Bandstruktur. Wir zeigen, dass zirkularer Dichroismus in der Winkelvertei
lung der Photoelektronen stark von der Geometrie des Experiments und der Energie der
Photonen abhängt. Nur unter speziellen Umständen ist es möglich zirkularen Dichoris
mus zu benutzen um experimentellen Zugang zum Bahndrehmoment und in Systemen
mit hoher SpinBahnWechselwirkung vielleicht sogar zur Spintextur der Oberäche zu
bekommen. Aufgrund des starken Einusses der Endzustände ist die Interpretation von
Dichroismusdaten höchst komplex und muss besonders vorsichtig durchgeführt werden.
Stichwörter: winkelaufgelöste Photoemissionzweidimensionale ElektronensystemeGraphenTopologischer IsolatorOberächenlegierungenStreuungsmechanismenCoulomb WechselwirkungBahndrehmomentSpintronik
vi
Contents
1 Introduction 1
2 Scientic Background 5
2.1 Electrons in low dimensions . . . . . . . . . . . . . . . . . . . . . . . . . . 5
2.1.1 Electrons in solids . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6
2.1.2 Surface states . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7
2.2 Spinpolarized surface states . . . . . . . . . . . . . . . . . . . . . . . . . . 8
2.2.1 The Rashba eect . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9
2.2.2 Topological insulators . . . . . . . . . . . . . . . . . . . . . . . . . 11
2.3 Surface states vs. 2D states . . . . . . . . . . . . . . . . . . . . . . . . . . 13
2.3.1 Surface alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14
2.3.2 Graphene . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15
3 Experimental Techniques 19
3.1 Photoemission spectroscopy . . . . . . . . . . . . . . . . . . . . . . . . . . 19
3.1.1 The photoemission process . . . . . . . . . . . . . . . . . . . . . . . 19
3.1.2 Quasiparticle picture . . . . . . . . . . . . . . . . . . . . . . . . . . 23
3.2 Angular resolved photoemission . . . . . . . . . . . . . . . . . . . . . . . . 25
3.3 Core level spectroscopy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 29
4 Coulomb interaction in topological insulators 31
4.1 Bi2Se3, Bi2Te3 and Bi2Te2Se . . . . . . . . . . . . . . . . . . . . . . . . . . 32
4.2 Doping behavior . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 33
4.3 Coulomb interaction at low charge carrier densities . . . . . . . . . . . . . 34
4.4 Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 38
vii
Contents
5 Surface band structure of TiTe1.5Se0.5 43
5.1 Search for new topological materials . . . . . . . . . . . . . . . . . . . . . . 43
5.2 Crystal structure . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 44
5.3 Electronic structure . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 45
5.4 Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 48
6 Scattering mechanisms in thallium doped epitaxial graphene 51
6.1 Impurities on graphene . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 52
6.2 Doping eect of Tl adatoms . . . . . . . . . . . . . . . . . . . . . . . . . . 53
6.3 Linewidth analysis and theoretical description . . . . . . . . . . . . . . . . 56
6.3.1 Longrange scattering . . . . . . . . . . . . . . . . . . . . . . . . . . 56
6.3.2 Shortrange scattering . . . . . . . . . . . . . . . . . . . . . . . . . 58
6.4 Graphene as topological insulator . . . . . . . . . . . . . . . . . . . . . . . 59
6.5 Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 61
7 Circular dichroism in the band structure of surface alloys 63
7.1 Circular dichroism in the angular distribution of photoelectrons . . . . . . 64
7.2 Photoemission experiments . . . . . . . . . . . . . . . . . . . . . . . . . . . 65
7.3 Theoretical description . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 67
7.4 Orbital angular momentum in surface alloys . . . . . . . . . . . . . . . . . 69
7.5 Photonenergy dependence . . . . . . . . . . . . . . . . . . . . . . . . . . . 70
7.6 Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 72
8 Summary and Outlook 75
8.1 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 75
8.2 Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 76
8.2.1 Topological insulators . . . . . . . . . . . . . . . . . . . . . . . . . 77
8.2.2 Circular dichorism measurements . . . . . . . . . . . . . . . . . . . 78
8.2.3 Graphene . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 78
viii
Chapter 1
Introduction
God made the bulk; surfaces were invented by the devil. [1] As the quote from Wolfgang
Pauli hypothesizes, the physics of surfaces is quite dierent compared to the bulk. One
reason for the dierent behavior is the dimensional constraints of the electrons. Since the
beginning of the 20th century it is known that in lowdimensional materials the limits of
classical physics are reached. As soon as the dimensions of an object are smaller than
the wavelength of the conduction electrons, quantum phenomena emerge. Surfaces can be
described as twodimensional electron systems (2DESs) where the electrons are conned in
one direction but can move freely in the plane. Some famous examples for physical eects
that can only be explained by a quantummechanical picture like the quantum Hall eect
are found in 2DES [24].
For investigation of such phenomena, accurate fabrication of lowdimensional materials
is required. The enormous development of technical knowledge and experimental methods
in the last decades allows scientists to design and investigate new lowdimensional systems
with fascinating properties that can be described by quantum mechanics. It is possible
to study materials at the nanoscale in real space with atomic force microscopy (AFM)
and scanning tunneling microscopy (STM). For determination of the atomic structure at
the surface low energy electron diraction is a very useful technique. To explore the
electronic structure at the surface xray photoelectron spectroscopy (XPS) and angular
resolved photoemission spectroscopy (ARPES) are the methods of choice. In this thesis,
the electronic properties of 2DESs localized at the surface are investigated using ARPES.
In particular, the focus of this thesis lies on topological insulators (TIs). TIs are
materials that have an insulating bulk but are conducting on their surface. The conduct
ing surface states are very interesting due to their spin polarization and their robustness
1
Chapter 1. Introduction
against defects. Many of them have a linear dispersion relation and are very promising
candidates for fast spintronic devices. Common theoretical descriptions of TIs are for
mulated in terms of singleparticle quantum mechanics [5]. Usually, the electronelectron
interaction is neglected since the dielectric constant in TIs is extremely high and the inter
action is eectively screened. However, the strength of the interaction is also dependent
on the charge carrier density. If the charge carrier density is low enough, electronelectron
interaction can play an important role  it can even turn the topological phase into an insu
lating ground state [6]. Therefore, it is a crucial issue to understand the interplay between
strong electronelectron interactions and the topological surface states. While studying
the Coulomb interaction in Bi2Te2Se it was found that the bands are substantially aected
by the electronelectron interaction. Depending on the charge carrier density the band
structure is renormalized and in addition an aginginduced band bending was observed.
Beside the detailed investigation of known TIs, it is also very important to look for new
topological materials. In this thesis rst results of an ARPES study of TiTe1.5Se0.5, which
is assumed to be a TI, are presented. Due to their high atomic spinorbit coupling (SOC)
strength transition metal dichalcogenides are very promising candidates for materials with
a topologically nontrivial surface state. Some theoretical studies predicted TiS2−2xTe2x
to turn into a TI for 0.48 < x < 0.80. To check if TiTe1.5Se0.5 behaves similarly the
rst ARPES measurements on this system were performed. The band structure looks
promising, but to identify the systems as a TI, further studies are necessary since the
assumed topological surface states are located in the unoccupied states.
In addition to TIs, epitaxial graphene on SiC(0001) was studied. It was shown that
chemical doping is an ecient method to tune the electronic structure and to shift the
Fermi level in either direction. However, every time dopants are deposited on graphene they
unavoidably introduce disorder and change the charge carrier mobility. A very important
issue for the development of future electronic devices based on impurities on graphene is the
ability to predict the involved scattering mechanisms and account for them accordingly. In
general, longrange scattering is said to be the dominant scattering mechanism in graphene
transport devices. For thallium atoms on graphene, which can be considered paradigm
longrange scatterers, signicant scattering contributions from shortrange scattering were
found. Using signatures of quasiparticle scattering in the photoemission spectral function
and a selfenergy model for both longrange and shortrange scattering mechanisms, Tl
adatoms could be identied also as ecient shortrange scattering centers.
In the third topic of this thesis, the use of circular dichroism (CD) measurements as
2
a method to access the orbital angular momentum (OAM) or even the spin of a surface
state is discussed. Surface alloys on the Ag(111) surface show a large spin splitting in
the surface states due to the RashbaBychkov eect [7]. Besides the great potential for
applications in the eld of spintronics, these alloys are also perfect test systems for surfaces
with giant spin splitting. By using circularly polarized light one can measure a CD signal
in the surface alloys on Ag(111). It was found that the CD signal is strongly dependent
on the photonenergy and does not directly contain information about the spin. Instead of
following the spin direction, CD is dominated by the geometry of the experimental setup,
by the dipole selection rules and by the nal state.
This thesis is organized as follows: In Chap. 2 an introduction to the scientic back
ground required for the understanding of the experimental results is given. Chap. 3 de
scribes the technical background and the experimental setups that were used to carry out
the experiments. The results from the studies about the electronelectron interaction in
TIs are presented in Chap. 4. In Chap. 5 the surface band structure of a titanium dichalo
genide is introduced. Chap. 6 is dedicated to our experimental results on Tl doped epitaxial
graphene. In Chap. 7 the possibility of accessing the spin orientation in surface states using
circularly polarized light in ARPES experiments is discussed. Finally, a detailed summary
of the main results is given in Chap. 8 and some ideas for future research projects based
on the previous chapters will be presented.
3
Chapter 1. Introduction
4
Chapter 2
Scientic Background
In solid state physics the main focus is on crystals and the investigation of their properties.
Scientists are interested in electrical, magnetic, optical, or mechanical characteristics. In
addition to the crystal structure, the electronic properties of a solid are of special interest.
The latter are determined by the electrons inside the crystal. Moreover the potential in
which the electrons are embedded plays a very important role. For example, electrons in
a lowdimensional environment behave quite dierent from free electrons.
2.1 Electrons in low dimensions
Generally, electrons in solids move in three dimensions, but by reducing the spatial char
acteristics of the crystal, for example, by creating surfaces or interfaces, electrons can be
forced to stay in less than three dimensions. If they are conned to certain directions or
planes, their energy E and momentum ~k in the relevant direction will be quantized. In
a quantum well, electrons are conned in only one direction, in a quantum wire they are
conned in two directions and in a quantum dot connement exists in all three directions.
The simplest case of electron connement is shown by an electron in a potential well
in one dimension. The potential well of the length L is shown in Fig. 2.1 (a) and can be
described by [8, 9]
V (x) =
0, for 0 < x < L
∞, else
Solving Schrödinger's equation for this potential gives the same dispersion relation as
5
Chapter 2. Scientic Background
E
x0 L
V(x)=∞ V(x)=∞
V(x)=0
barrier well barrier
(a) (b)
k
E4
E3
E2
E1
k1 k2 k3 k4
Figure 2.1: Onedimensional quantum well: (a) Outside the onedimensional well the barriers have innitely large potential, while inside the potential is zero. (b) The energy of anelectron in a onedimensional quantum well (black circles) and a free electron (red line), bothdepend on the wave vector in the same way [see Eq. 2.1]. However, the electron in the wellmay only have certain, discrete energy levels.
for free electrons
E(~k) =~2~k2
2m(2.1)
but for the potential well there are only discrete momentum values allowed that satisfy
k = nπ/L with n ∈ N [see Fig. 2.1 (b)]. ~ represents Planck's constant h divided by 2π
and m is the mass of the electron.
Conned electron systems are of particular interest because they give access to special
physical phenomena that are based on quantum physics. Particularly, in two dimensions i.e.
at surfaces or interfaces, many interesting physical eects can happen, like the (fractional)
quantum Hall eect [10]. In this thesis we are focusing on electrons at surfaces, i.e. on
2DES.
2.1.1 Electrons in solids
In a very simple picture solids can be modeled by atoms of the same kind that come close
together. Electrons in solids feel a periodic potential V (~r) = V (~r + ~R) where ~R gives the
lattice periodicity [8]. The solutions for the Schrödinger equation with such a potential
are Bloch waves Ψk(~r) = uk(~r)ei~k~r with uk(~r) = uk(~r + ~R). Accordingly, also the energy
eigenstates show periodic behavior and the free electron parabola is duplicated at every
lattice vector, as shown schematically in Fig. 2.2 (a) and (b).
Since the band structure is periodic in ~R it is sucient to draw the bands only in the
6
2.1. Electrons in low dimensions
Momentum
Ene
rgy
Momentum
(a) (b) (c)
π/a π/a
Momentum
π/a π/a2π/a 2π/a0
Figure 2.2: Electronic band structure for electrons in a periodic potential: (a) The freeelectron parabola. (b) Periodic zone scheme of the band structure in a solid. (c) Reducedzone scheme in the rst Brillouin zone.
rst Brillouin zone like in Fig. 2.2 (c). Due to the lattice potential small energy gaps will
be opened at the crossing points which lead to the electronic band structure that consists
of the allowed bands and band gaps [not shown in Fig. 2.2].
2.1.2 Surface states
As shown in Sec. 2.1.1 the solutions to the Schrödinger equation in an innite crystal are
Bloch waves. By creating a surface the potential deviates from its perfect periodicity. For
a potential that is not perfectly periodic there are additional solutions for the Schrödinger
equation that can be divided into two groups: (i) the Bloch waves, which decay expo
nentially into vacuum [see Fig. 2.3 (a)] and (ii) states, which are damped exponentially
into the vacuum as well as into the bulk. The latter are the socalled surface states and
are schematically drawn in Fig. 2.3 (b). Their energy eigenvalues are located in the pro
jected bulk band gap and their wave vector k is imaginary. Electrons within these surface
states are strongly conned in the direction perpendicular to the surface, whereas they can
propagate freely within the surface. Therefore, surface states constitute a 2DES.
In the discussion of surface states one distinguishes Shockley states from Tamm states
[11]. In principle both are terms for the description of the same physical phenomenon,
i. e. surface states but the mathematical approach is dierent. Shockley surface states are
described in the framework of the nearly free electron model for clean and ideal surfaces and
exist simply due to crystal termination at the surface [12]. In contrast, the Tamm states
7
Chapter 2. Scientic Background
bulk vacuum
bulk state
bulk vacuum
surface state(a) (b)
Figure 2.3: (a) In a semiinnite crystal the Bloch waves are exponentially damped in thevacuum region. (b) Due to the missing periodicity at the surface there are additional solutionsto the Schrödinger equation, which have imaginary wave vector. They decay exponentiallyinto vacuum as well as into the bulk.
are obtained using the tight binding model. The existence of Tamm surface states implies a
considerable perturbation of the potential in the surface region due to reconstruction [13].
In addition to these surface states, there are surface resonances that decay exponentially
into vacuum but show a sizable amplitude in the bulk.
2.2 Spinpolarized surface states
In general, in a threedimensional (3D) solid time reversal [E(↑, ~k) = E(↓,−~k)] as well
as spatial inversion symmetry [E(↑, ~k) = E(↑,−~k)] are fullled. The combination of both
gives rise to Kramers spin degeneracy [14], expressed as
E(↑, ~k) = E(↓, ~k)
However, SOC can lift the spin degeneracy if one of the symmetries is broken [15].
In current surface science research, there are two main classes of spinpolarized surface
states [16,17] that are of interest; Rashbasplit surface states and the surface states in TIs.
In the next two sections both will be introduced and compared to each other.
8
2.2. Spinpolarized surface states
2.2.1 The Rashba eect
The spatial inversion symmetry of a solid can be easily broken, for example, due to bulk
inversion asymmetry in noncentrosymmetric semiconductors. As a consequence of SOC the
spin degeneracy can be removed [1820]. Also, a structural inversion asymmetry, which is
caused simply by the presence of the surface in a semiinnite crystal, breaks space inversion
symmetry. Electronic states at the surface feel the structural inversion asymmetry and
become spinpolarized due to SOC. The case in two dimensions (2D) is usually considered
as the Rashbaeect [7,21]. For the theoretical description of the spin splitting in a 2DES
with inversion asymmetry along the zdirection, the Rashba Hamiltonian is added to the
quasifree 2D electron gas conned in the (x; y)plane. The Hamiltonian describes SOC in
propagating electronic states and is given by
HRB = αR~σ(~k × ~ez) (2.2)
with the Rashba parameter αR determined by the potential gradient perpendicular to the
2DES, the Pauli matrices ~σ = (σx, σy, σz), the electron momentum in the plane ~k and the
unit vector ~ez perpendicular to the plane of the 2DES. Solving the Schrödinger equation
for the Rashba Hamiltonian gives
E(k) = E0 +~2k2

2m∗± αRk = E0 +
~2
2m∗(k ± kR
)2
for the energy dispersion. The resulting band structure consists of two parabolas with
an eective mass m∗, which are shifted by the momentum oset ±kR = αRm∗/~2 from
the original momentum. However, at high symmetry points the dispersion has to be spin
degenerate because of time reversal symmetry. A typical dispersion is schematically drawn
in Fig. 2.4 (a) and (b).
A third characteristic parameter that results from the momentum oset kR is the so
called Rashba energy ER = ~2k2R/(2m
∗) = m∗α2R/(2~2). It describes the energy dierence
between the band extremum and the crossing point at the high symmetry point. A cut
through the band structure at a constant energy above the crossing point gives two concen
tric circles [see Fig. 2.4(c)]. Due to the vector product in Eq. 2.2 the spin vector is expected
to be entirely inplane, i.e. perpendicular to ~ez and perpendicular to the momentum k
of the electron. Consequently the spin vector points tangential along the constant energy
contours; it rotates clockwise on the inner circle and counterclockwise on the outer one.
9
Chapter 2. Scientic Background
Wave Vector k
ER
kRαR>0
Initi
al S
tate
Ene
rgy
E
Wave Vector k
αR=0(a) (b) (c)
Figure 2.4: Energy dispersion of a 2D electron gas (a) without and (b) with Rashba SOC.The characteristic parameters of the model, ER and kR, are marked. (c) Spin polarisation ona constant energy contour above the crossing point.
However, in total the system is not magnetic since an integration over the whole reciprocal
space gives no net spin.
The rst example for a Rashbasplit surface state is the one on Au(111). LaShell et
al. [22] observed an energy splitting that is proportional to the wave vector and about
110meV at the Fermi level. Dierent approaches have been chosen to tune [23] or to
enhance the spin splitting for example by adsorption of Ar, Kr or Xe [24].
In order to be able to manipulate the spin splitting at the surface in a desired fashion,
it is very important to understand the underlying mechanism. In a very simple picture
the spinsplitting of the 2D states caused by the Rashba eect can be seen as a spin
polarization due to the Zeemann eect. The eective magnetic eld Beff would be ~k
dependent and described by αR(~k × ~ez). The direction of Beff , i.e. the spin quantization
axis, would be given by the vector product and the size of the splitting is determined by
the Rashba constant αR, which is proportional to the gradient of the potential conning
the electrons to the surface. But within the framework of the quasifree electron model
typical values for the spin splitting would be several orders of magnitude smaller than
experimentally observed [25, 26]. Using a simple tight binding model it was shown [25]
that αR is proportional to the atomic SOC and an asymmetry parameter γ.
Recently, it was proposed by Park et al. [27] that the Rashbatype spinsplitting is a
consequence of the existence of local OAM. The local OAM is the quantum number given
10
2.2. Spinpolarized surface states
by the orbital angular momentum operator L, often called the magnetic quantum number.
The OAM produces an asymmetric charge distribution by inducing small dipoles. The
electric eld perpendicular to the surface aligns the electric dipole and results in chiral
OAM states and the spin splitting. The characteristic chiral spin structure is formed
through SOC and is claimed to be a consequence of the chiral OAM. The authors show
that by considering the OAM as the origin of the spin splitting the predicted size of the
spin splitting is much closer to the measured value. They conrm by them that the atomic
SOC size plays an important role.
In addition to the eort towards a theoretical understanding, it was found that the spin
splitting can be enhanced by corrugation of the surface potential and outward relaxation
of some atoms [28]. It is also possible to transfer the spinpolarized surface states on
a semiconducting substrate [29]. The main goal in the eld of spintronics is to tune
the spin splitting via an external electrical eld. The Rashba eect on semiconducting
substrates seems to build the basis for many dierent electrical devices like the spin eld
eect transistor of Datta and Das [30].
2.2.2 Topological insulators
The surface states in a 3D TI constitute another spinpolarized 2DES that is discussed in
this section. A TI is a material that has an energy gap in its bulk but is conducting at the
edges. In three dimensions, the bulk itself is insulating but the surfaces are metallic. There
are also 2D TIs, which have onedimensional gapless edge states. As explained in Sec. 2.1.2
surface states exist in the energy band gap of the bulk material. There are topologically
trivial and nontrivial surface states. The nontrivial ones are called topological surface
states. Trivial surface states arise from and end in the same bulk band and they exist also
in projected bulk band gaps. Topological surface states, however, connect two dierent
bulk bands and the corresponding band gap is a true bulk band gap. In addition, this
band gap is inverted, which means that the order of conduction and valence band in a TI
is reversed compared to the band structure of trivial materials. By connecting a TI with a
normal insulator like, for example, vacuum the topology of the band structure changes at
the interface. In order to restore the order of the bulk bands the band gap will be closed
and reopened, which results directly in metallic edge states at the surface.
In general, the surface states in a TI are Diraclike and show conical dispersion but
in contrast to graphene the bands are spinpolarized because of the strong SOC. The
broken inversion symmetry at the surface dictates the spinsplitting of the surface states.
11
Chapter 2. Scientic Background
Timereversal symmetry gives rise to the socalled spinmomentum locking; all electrons
with spin up (down) travel to the right (left) side. Accordingly, chiral spin textures are
found in momentum space with the sense of chirality reversed across the Dirac point.
Electrons in the surface states are immune to back scattering from disorder and non
magnetic impurities, since for back scattering the electron would need to ip also its spin.
Due to this fact, such surface states are extremely robust to disorder and they are called
'topologically protected'. An idealized band structure for a TI is shown in Fig. 2.5. The
simplest criterion to identify topologically nontrivial surface state is an odd number of
Fermi level crossings between the Brillouin zone center and the boundary. In the simple
example in Fig. 2.5, it would be just one crossing.
Fermi level
Momentum
Ene
rgy
conduction band
valence band
Figure 2.5: An idealized band structure for a topological insulator. The Fermi level fallswithin the bulk band gap which is traversed by topologicallyprotected surface states.
A TI in 2D is also known as a quantum spin Hall insulator. This state was theoretically
predicted in 2005 [31] for graphene at low temperatures. Since the SOC in carbon atoms
is very small, the predicted gap is only of the order of some µ eV and experimentally not
observable. Subsequently, Bernevig et al. [32] claimed that there is a quantum spin Hall
state in HgCdTe quantum well structures. One year later the rst experimental observation
of a TI was reported in that system [33]. Several materials of 2D TIs have been proposed
theoretically [31,32,34].
Theoretical predictions about topological surface states were also made for several 3D
materials [35, 36] like Bi1−xSbx and strained HgTe and αSn [37]. The rst experimental
discovery of a 3D TI was reported in 2008 by Hsieh et al. [38]. For Bi1−xSbx ve Fermi
level crossings were found.
Shortly later many theoretically predictions for simpler versions of 3D TIs were pub
lished. For example, Bi2Te3, Sb2Te3 [39] and Bi2Se3 [40] should show a large bulk band
12
2.3. Surface states vs. 2D states
gap and a gapless surface state consisting of only one single Dirac cone at the Brillouin
zone center. Indeed, the linear dispersion relation of these surface states were subsequently
observed in ARPES experiments [40, 41]. Since then, the eld has expanded at a rapid
pace [4246]; many new compounds are predicted to be topologically nontrivial [47, 48]
and some already experimentally proven [5, 49,50].
One obstacle in real TIs is the high conductivity of the intrinsically doped bulk due
to unavoidable defects and vacancies formed during the growth procedure. In Bi2Se3, for
example, Se vacancies are responsible for the doping level of the bulk. The challenge in
every experiment is to distinguish between surface and volume eects. For transport mea
surements in highly doped TIs, dierentiation can be quite dicult or even impossible.
Therefore, a TI with a large bulk band gap and the Fermi level inside the gap would be
desirable. There are dierent approaches to solve this problem like, for example, reducing
bulk carrier density by doping [51,52]. One possibility is to mix the elements and get ma
terials that fulll the requirements, like Bi2Te2Se [5355]. Another option is to reduce the
thickness of the sample in order to increase the surfacetovolume ratio. For such nanofab
rication three main methods are used; mechanical exfoliation [56], growing nanoplates
and nanoribbons by vaporliquidsolid synthesis [57], and growth of TI nanostructures by
molecular beam epitaxy (MBE). The last approach allows for layer by layer growth with
large areas, high crystalline quality, and accurate thickness and chemical composition from
one to several quintuple layers (QLs) [58].
The surface states of TIs are not only of fundamental importance but have also great
potential applications. Despite disorder due to impurities they are predicted to stay metal
lic even at T = 0 because of forbidden back scattering [59]. Due to the dissipationless
transport the edge states of TIs are of huge interest for room temperature spinbased
electronic devices [60] and applications in quantum computation [46, 61]. In addition, the
helical surface states of TIs could provide access to novel physical phenomena like Majorana
fermions [62].
2.3 Surface states vs. 2D states
In addition to topological surface states, we investigated 2DESs of two other types. We had
a closer look at the electronic structure of surface alloys on Ag and we studied the eect of
impurity scattering in the band structure of graphene. All systems of interest in this work
are treated as 2D but the way they are fabricated and their resulting properties are quite
13
Chapter 2. Scientic Background
dierent. Surface alloys on Ag, for example, show spin splitting due to the Rashba eect
and the graphene band structure is spin degenerate. Building a surface alloy on Ag shows
consequences for the rst few atomic layers at the surface whereas graphene, being exactly
one atom thick, is a perfect 2D crystal. The electrons in graphene behave like massless
particles while the electronic states in the surface alloys show parabolic dispersions. In the
following section both systems are introduced and their basic principles and properties are
presented.
2.3.1 Surface alloys
Surface alloys on Ag(111) are known for their huge Rashbatype spin splitting in the surface
states [63, 64]. For the preparation of the surface alloys a third of a monolayer of Bi or
Sb is deposited on the clean Ag(111) surface. Every third atom in the Ag(111) surface is
replaced by an alloy atom and a long range ordered surface alloy is formed. The resulting
(√
3×√
3)R30 structure is shown in Fig. 2.6.
(a)
Δz
(b)
Figure 2.6: Surface alloys on Ag(111): (a) Top view and (b) side view of the (√
3×√
3)R30
structure formed by surface alloys. Every third silver atom (grey) is replaced by an alloy atom(red). The relaxation out of the surface plane is described by ∆z.
The band structure of the surface alloys has been extensively investigated and discussed
in literature [28,65]. The dispersion shows two spinpolarized bands with the characteristic
momentum oset kR. The surface alloy Bi/Ag(111) shows a huge spin splitting of ER =
200meV. The spinsplitting mechanism and the origin of the huge Rashba energies is
not completely understood but it was shown that there are three important ingredients;
structural inversion symmetry, atomic SOC and the outward relaxation of the alloy atoms.
With increasing relaxation ∆z the asymmetry grows and the resulting spin splitting gets
larger [25, 28, 66]. It was theoretically shown that the orbital character of the bands is
determined by the relaxation, which varies for dierent alloy atoms.
In addition to the orbital character, the spin structure is aected by the corrugation
of the surface potential. Surface alloys show not only inplane but also outofplane spin
14
2.3. Surface states vs. 2D states
components [64,67]. This can be explained by an inplane inversion asymmetry that results
in an inplane component of the potential gradient at the surface [68].
All these extra features of the spin splitting are not included in the original Rashba
model. However, for building spintronic devices it would be very desirable to have one
combined theory describing all ingredients and features of the spin splitting mechanism. A
more detailed understanding of tuning the spin splitting would allow one to fabricate all
dierent kinds of devices with the proper spin textures for any application.
2.3.2 Graphene
The last candidate for a 2DES in this work is the perfect 2D crystal found in the carbon
allotrope graphene. It is one single atomic plane of graphite and consists of sp2 bonded
carbon atoms arranged in a honeycomb lattice.
The theoretical description of a single layer of graphite was already presented in 1947
by P. R. Wallace [69], but it was believed for a long time that it would be very unstable
and impossible to isolate. In 2004, Novoselov and Geim succeeded in isolating a single
layer of graphene. They used the micromechanical exfoliation procedure, also known as
the 'Scotch tape technique' and transferred the graphene sheet onto a SiO2 substrate
[70]. After the successful experimental isolation of graphene the research on this material
increased rapidly. Many interesting eects could be shown like, for example, the anomalous
integer quantum Hall eect in graphene [71, 72]. Single layers of graphite were known
before, but the breakthrough was given by the fact that graphene on SiO2 shows an optical
contrast that makes it easy to dierentiate single and double layer graphene. For their
groundbreaking experiments regarding the twodimensional material graphene Novoselov
and Geim received the Nobel prize in physics in 2010.
The electrons in graphene behave like massless particles and can be described by the
Dirac equation. Due to the presence of two equivalent sublattices [see Fig. 2.7(a)], the wave
function shows 2spinor character and determines the electronic properties. Graphene has
two πbands that touch each other exactly at the Fermi energy at the Kpoints the
six corners of the Brillouin zone [Fig. 2.7(b)] and behaves like a semimetal. These points
are the socalled Dirac points. Close to those points, the bands disperse linearly and the
band structure has the shape of a cone [see Fig. 2.7(c)], where the band velocity is about
vF ≈ 106 m/s. The dispersion can be described by the following equation:
E(k) = ~vFk
15
Chapter 2. Scientic Background
(a) (b)
Γ K
M
K'
kx
ky
(c)
Figure 2.7: Structure of graphene: (a) two equivalent sublattices shown in red and blackresult in graphene's honeycomb lattice, (b) the corresponding hexagonal Brillouin zone withthe most important high symmetry points indicated. (c) Close to the Kpoint the bandstructure can be approximated by a cone.
Current research on graphene can be divided into two section. One is dealing with the
fundamental properties and interesting quantum eects that can be observed in graphene.
The other section is involved in pushing graphene further in the direction of applications in
electronic devices. But in this eld, there are some major problems and questions to solve:
It is still not clear what causes the minimum conductivity of 4 e2/h in graphene [73, 74].
A possible explanation could be the charge puddles in graphene sheets that give rise to
higher scattering rate [75]. Another problem is the missing energy band gap in graphene
and the resulting low ratios between the 'on' and 'o' state in a eld eect transistor built
out of graphene [73].
Graphene production
In principle, there are three main approaches to produce graphene [9]: Pulling one single
layer from graphite, which is known as mechanical exfoliation, or growing a layer of carbon
on a substrate either via epitaxial growth or via chemical vapor deposition (CVD).
Exfoliation: To get one single layer of graphene by exfoliation, multiple peeling steps
with an adhesive tape until only one is left are required. After cleaving, the akes are
transferred onto a SiO2 substrate where the number of layers can be determined with
an optical microscope. This method results in akes with a lateral size of about one
millimeter [76]. Exfoliated graphene samples show very high quality and high charge
carrier mobility and are the best for proofofprinciple devices in basic research. However,
this technique is not suitable for large scale production of graphene.
16
2.3. Surface states vs. 2D states
Epitaxy: Graphene can be grown on various metallic substrates by CVD or epitaxially
on a semiinsulating substrate like silicon carbide (SiC) by high temperature annealing.
Already decades before the discovery of graphene in 2004, it was known that hydrocarbons
can be cracked on catalytic metal surfaces. In particular, it was shown that CVDgraphene
grows well on Ni [7779], Rh [80], Ru [80], Ir [81,82] and Pt [80,83,84]. The advantage of
that method is the selflimiting character which leads exactly to one layer of carbon atoms.
However for many applications the metallic substrate is undesirable.
A more promising way to build graphene devices on a large scale is the epitaxial growth
on SiC wafers. Silicon has a higher vapor pressure and leaves the carbon atoms at the
surface. By heating a SiC wafer to temperatures above 1100C in ultra high vacuum (UHV)
graphene is formed on the surface [85]. Its thickness, electron mobility and charge carrier
density depends very much on which side of the SiC wafer is used for graphene formation.
The growth on SiC(0001) the carbonterminated or Cface results in rotationally
disordered multilayer graphene due to the weak interaction between the graphene layers
and the substrate. Due to this rotational disorder the layers are electronically decoupled
and show pretty high carrier mobilities that are comparable with isolated graphene sheets
[86,87]. However, controlling the thickness is quite limited on that side [88,89].
On the opposite side the siliconterminated or Siface graphene grows in large
sheet and covers whole terraces [8992]. However, the commercially available SiC wafers
have typically a lot of scratches on this surface, which have to be removed by hydrogen
etching at elevated temperatures. After etching away several hundred nanometers the
surface show large and clean terraces with a width of 1500Å and a step height of only one
unit cell [93,94]. The following annealing step can either take place in UHV or in 900mbar
Ar. Graphitization of SiC in UHV is accompanied by a considerable roughening of the
surface. This can be avoided by annealing in Ar at elevated temperatures, which results in
step bunching and much larger terraces [95]. In both cases, the rst carbon layer that is
formed has a honeycomb structure, but does not show graphenelike electronic properties.
Since every third atom of the carbon layer is sp3 hybridized and covalently bound to the
substrate the πbands cannot be formed [96]. The growth process is schematically drawn
in Fig. 2.8.
In addition, this socalled zerolayer forms a (6√
3 × 6√
3)R30 reconstruction with
respect to the SiC substrate [88, 91, 98100]. With increasing temperature further carbon
layers will be formed. The second carbon layer is called monolayer graphene [see Fig.
2.8 (b)] and shows a Dirac cone at the Kpoint. However, the band structure contains
17
Chapter 2. Scientic Background
Figure 2.8: Side view models for (a) the (6√
3 × 6√
3)R30 reconstruction of SiC(0001)(called zerolayer) and (b) epitaxial monolayer graphene (taken from [97]).
signatures of the substrate. Due to charge transfer from the substrate to the graphene layer
the Dirac point is about 420meV below the Fermi level [97,101103] and the charge carrier
mobility is quite low compared to exfoliated graphene [104]. Since nucleation of a new
graphene layer starts at step edges, Arannealed samples are much more homogeneously
covered [95]. By choosing the right annealing temperature and duration the number of
graphene layers can be controlled quite easily.
18
Chapter 3
Experimental Techniques
3.1 Photoemission spectroscopy
Photoemission spectroscopy (PES) is based on the photoelectric eect discovered by H.
Hertz in 1887 [105]. About 20 years later Einstein was able to explain this eect by
postulating the quantum nature of light [106], for which he was awarded the Nobel prize in
physics in 1921. In the following sections an introduction to this experimental technique
and a theoretical description are given.
3.1.1 The photoemission process
Light exists as discrete quantized packets called photons, with an energy ~ω. If they
impinge on a surface and their energy is larger than a characteristic value Φ, called the
work function, they release electrons with kinetic energy Ekin from the surface. If Ekin is
measured by an analyzer, the binding energy EB of the electron can be determined via
EB = ~ω − Φ− Ekin (3.1)
For photoemission measurements the work function of the spectrometer has to be used.
Sample and spectrometer are usually in electrical contact and thus the Fermi level is
aligned. All relevant energies involved in the photoemission process are shown in Fig. 3.1.
Note that EB is referenced to the Fermi level (EF is equivalent to zero binding energy),
while the kinetic energy is measured with respect to the vacuum level. Depending on
the energy of the incident photons there are two dierent types of photoemission spec
troscopy experiments: For the excitation of valence electrons, photons in the ultraviolet
19
Chapter 3. Experimental Techniques
Evac
EF
N(E)
Evac
EF
EB
core levels
valence band
ΦS ΦA N(E)
hν
hν
PES spectrumEkin
sample
Figure 3.1: Schematic illustration of the energies involved in a photoelectron emission process from a solid. N(E) is the energy distribution of the photoemitted electrons. After [107].
(UV) range are used (ultraviolet photoemission spectroscopy, UPS) whereas the use of
xrays gives access to the core levels, electronic states with much higher binding energy
(xray photoemission spectroscopy, XPS).
Since Eq. 3.1 is only valid for electrons that did not experience any inelastic event
while leaving the material, the probing depth of those techniques can be estimated by the
mean free path λ of the electrons which gives the average distance electrons travel without
energy loss. It is a measure for the escape depth of the electrons in a solid. For the relevant
energies in PES the electrons can be described as a free electron gas. In this case λ depends
only on the electron concentration. Since this is roughly equal in all materials the mean
free path follows a universal curve that is shown in Fig. 3.2. This curve can be described
20
3.1. Photoemission spectroscopy
1
2
4
6
10
2
4
6
100
mea
n fr
ee p
ath
(Å)
100
101
102
103
104
energy (eV)
Figure 3.2: Universal curve: Mean free path as function of energy, calculated using Eq. 3.2.The escape depth of the electrons in a solid is almost independent of the material. For therelevant energies the mean free path is about several Å.
by the phenomenological function [108]
λ(E) =538
E2+ 0.41
√aE (3.2)
where a is the thickness of a monolayer in nm. The curve has a broad minimum in the
energy range of 50100 eV. Using those energies for PES means that the escaping electrons
originate from the rst few atomic layers at the surface. This makes PES a very surface
sensitive technique.
The photoemission of an electron [Eq. 3.1] can be described in a simple picture as
follows: A photon impinges on a surface of a solid and excites an electron via the photo
electric eect. The excited electron escapes into the vacuum while energy and momentum
have to be conserved. Since the photon momentum is small compared to the momentum
of the electron ~k, it can be neglected. The resulting direct transition is possible in a crystal
lattice, where a lattice vector can compensate for the missing momentum [compare Sec.
2.1.1]. For a quantitative interpretation of photoemission experiments a more elaborate
picture of the photoemission process is needed.
There are two basic approaches to describe the photoemission process theoretically:
The rather simple threestep model and the more realistic onestep model. The following
theoretical description is based on the references [9, 107, 109]. Within the framework of
the threestep model the process is decomposed into three independent steps; (1) electron
21
Chapter 3. Experimental Techniques
excitation, (2) electron propagation to the surface and (3) escape through the surface
into vacuum [see Fig. 3.3]. Here it has to be pointed out that only elastically scattered
electrons are of interest since only those carry information about the initial state in the
solid. The measured photocurrent I is proportional to the product of the probability of the
photoexcitation, the probability of the electron traveling to the crystalvacuum interface
without being scattered, and the transmission function for the interface.
The separation into three independent steps is somewhat articial. In the socalled
onestep model this is eliminated and the whole photoemission process is considered as one
single step. It describes the excitation from an initial Bloch state into a damped nal state
near the surface. This damping takes care of the short mean free path of the electrons in
a solid.
E
Ef
Ei
0z
excitation
propagation escape
1
23
Figure 3.3: Schematic drawing of the threestep model. The photoemission process is dividedinto three steps; (1) photoexcitation, (2) electron propagation to the surface and (3) escapethrough the surface into vacuum.
The calculation of the photocurrent is based on Fermi's Golden Rule. For making the
calculation feasible the sudden approximation [107] is mostly used. Here, the electron
is assumed to immediately exit the surface of the material, without interacting with the
remaining electrons and the photohole it leaves behind. The photocurrent is then propor
tional to the transition probability ωfi from the initial Ψi to the nal state Ψf . Using the
dipole approximation gives [107]
I ∝ 2π
~〈Ψf  ~A~pΨi〉2δ(Ef − Ei − ~ω)
22
3.1. Photoemission spectroscopy
To simplify the transition matrix element a oneelectron view is taken for the initial
and nal state wave function. The initial state can be written as a product of the orbital
Φi,~k from which the electron is excited, and the wave function of the remaining electrons:
ΨNi = Φi,kΨ
ki (N − 1)
Accordingly, the nal state is written as a product of the wave function of the pho
toemitted electron Φf,Ekinand that of the remaining (N − 1) electrons:
ΨNf = Φf,Ekin
Ψkf (N − 1)
The square of the absolute value of the wave function of the remaining electrons gives
the spectral function, i.e.∑〈Ψk
f (N − 1)Ψki (N − 1)〉2 = A(~k,E), and the photocurrent
turns into
I ∝∑f,i,~k
〈Φf,Ekin~rΦi,k〉2A(~k,E)f(E, T )
where f(E, T ) = (eβ(E−µ)+1)−1 is the FermiDirac distribution function that accounts
for the occupation of the electronic states with β = (kBT )−1, the Boltzmann constant kBand the chemical potential µ. The spectral function can be related to the single particle
Green's function G(~k, E) via
A(~k,E) =1
πIm(G(~k, E)
)The Green's function for a system with noninteracting electrons is given by the formula
G0(~k,E) = 1/(E − E0~k− iγ), where γ is a innitesimally small number and E0
~kis the
dispersion E0~k
= ~2~k2/(2m∗). The corresponding spectral function in this case is a δ
function A0(~k, E) = 1πδ(E − E0
~k).
3.1.2 Quasiparticle picture
So far, all formulas were based on the independent electron approximation, which cov
ers a single electron moving in an eective potential Ueff (~r) of the atomic cores and the
remaining (N − 1) electrons with the resulting bare band dispersion E0~k. For a complete
description of an electron in a solid, one has to account also for manybody eects, resulting
in the independent electron picture breaking down. However, the properties of a system
with interacting electrons, called a 'Fermi liquid', can be mapped onto those of a system
23
Chapter 3. Experimental Techniques
of noninteracting electrons by a formalism of Landau. The bare electron combined with
manybody interactions are handled as new particles, socalled 'quasiparticle'. The main
conclusions of the independent electron approximation remain valid. The spectral proper
ties measured by photoemission spectroscopy of a Fermi liquid dier in four respects from
the free electron gas [107]: (1) The energy of the interacting system (E~k) is renormalized
relative to that of the noninteracting system (E0~k). (2) The quasiparticles have a nite
lifetime. (3) There is an incoherent background due to electronhole pairs. (4) The height
of the Fermi step is reduced.
In systems where manybody interactions are taken into account, it is useful to introduce
the socalled selfenergy Σ(~k,E), which accounts for the renormalization of the electron
energy. The Green's function turns into G(~k, E) = 1
E−E0~k−Σ(~k,E)
and the spectral function
for an interacting system is given by
A(~k,E) =1
π
Im(
Σ(~k, E))
[E − E0
~k−Re
(Σ(~k,E)
)]2
+[Im(
Σ(~k,E))]2 (3.3)
In the simplest case, Im(Σ) is constant and Re(Σ) = 0. The spectral function is then
a Lorentzian at E0~kwith full width at half maximum Γ = 2Im(Σ). The real part of Σ
causes deviations from the bare energy dispersion E0~kand the imaginary part is responsible
for the linewidth. The latter includes the intrinsic linewidth as well as broadening due to
interactions. E0~kis solely determined by the symmetries of the lattice potential. All the
inuences of manybody interactions like electronelectron and electronphonon scattering
can be expressed in terms of the complex selfenergy Σ.
With ARPES one yields information about the properties of the quasiparticles, i.e.
one measures the renormalized dispersion. Due to the high resolution of stateoftheart
analyzers a very accurate determination of the photoemission linewidth is possible and
ARPES became a powerful tool for the investigation of manybody interactions in solids.
For two or onedimensional electronic states the measured linewidth corresponds to the
width of the hole state and equals the imaginary part of the selfenergy. In this case
the fullwidthathalfmaximum (FWHM) of the photoemission peaks is related to the
quasiparticle lifetime τ via τ = ~/Γ. The quasiparticle lifetime is a sum of three main
contributions
Γ = Γe−e + Γe−ph + Γe−imp
where Γe−e is the electronelectron scattering, Γe−ph the electronphonon scattering and
24
3.2. Angular resolved photoemission
Γe−imp the impurity scattering [110].
For an electron at the Fermi level, Γe−e = 0 when T = 0, which means there is no phase
space for any scattering events and the lifetime of the electron is innite. At energies
E < EF , the scattering rate is proportional to (E −EF )2. At nite temperature there will
be partially occupied electronic levels in a shell of width kBT about EF . The scattering
rate is then proportional to (kBT )2. The total scattering rate due to electronelectron
interaction is therefore
Γe−e = 2β[(πkBT )2 + (E − EF )2] (3.4)
with the electronelectron interaction constant β. In the case of electronphonon scat
tering not only the lifetime is aected but also the energy dispersion. The band renormal
ization due to electronphonon scattering can be expressed as a change of the electronic
velocity v(k) = 1/~(∂E/∂k). The renormalized velocity can be calculated via [111]
v(k) =1
1 + λv0(k)
with the velocity of the noninteracting case v0(k) = 1/~(∂E0/∂k) and the electronphonon
coupling constant λ. Electronphonon interactions decrease the slope of the dispersing
bands and lead to a kink around the Fermi level. The contribution to the linewidth due
to scattering at impurities is independent of energy E and temperature T . It is a constant
contribution (Γe−imp = const.) and changes only with impurity concentration.
3.2 Angular resolved photoemission
With an angular resolved photoemission experiment it is possible to determine the angular
dependence of photoemitted valence band electrons as a function of their binding energy.
Therefore, not only the kinetic energy Ekin, but also the emission angle θ of the photoelec
tron is measured. When the photoexcited electron passes through the surface into vacuum
a freeelectron like nal state with Ekin = p2/2m is assumed. While escaping, the electron
momentum perpendicular to the surface is changed but the inplane component k is con
served. According to Fig. 3.4 k can be determined directly from the emission angle θ of
the photoelectron via
k [Å−1] =
√2meEkin
~2sin(θ) = 0.512
√Ekin [eV] sin(θ)
25
Chapter 3. Experimental Techniques
where me is the electron mass and θ the angle between k and normal emission. The
binding energy of the electron in the initial state is determined as before using Eq. 3.1.
vacuum
crystalθi
θ
z
k,int
k,ext
k ,int
kint
k ,ext p/h
k,int =k,ext =p/h
Figure 3.4: Relations between the crystal momentum and the measured electron momentumin the freeelectron nal state approximation.
The setup for an angular resolved photoemission spectroscopy (ARPES) experiment
consists of a photon source in the UV range and an electrostatic analyzer that measures
Ekin and θ. The photon source can either be a gas discharge lamp, a laser or synchrotron
radiation. The typical beam spot size of a UV source is 1mm2, whereas at the synchrotron
the illuminated area can be much smaller and the intensity much higher. Concerning the
analyzer, the availability of 2D chargecoupled device (CCD) detectors has made ARPES
an extremely detailed and precise tool to directly measure the electronic band structure
(EB(k)) of a 2DES. A typical setup is shown in Fig. 3.5. The inplane momentum can be
varied by turning the sample around θ and Φ, respectively, as indicated.
For the analysis of photoemission data the 2D spectra are usually divided into ei
ther momentum distribution curves (MDCs) or energy distribution curves (EDCs). While
MDCs show the photocurrent as a function of the emission angle at a constant binding
energy, EDCs display the measured intensity at a constant emission angle dependent on
the binding energy. For quantitative conclusions an appropriate background has to be
subtracted from the spectra. Therefore, the spectrum is divided into a primary spectrum
and a secondary spectrum where the latter represents inelastic events like electronelectron
and electronion scattering [107]. There are several sophisticated formulas for backgrounds,
like for example the version given by Tougaard [112], but usually it is sucient to apply
a constant background that accounts for the dark count rate in the detector plus the so
called Shirley background BS(E). This type of background is proportional to the weight
26
3.2. Angular resolved photoemission
UV photonshν
ph
otoe
lect
ron
s
hemispherical analyzer
2D detector
sample
Φ
θ
Figure 3.5: Typical angular resolved photoemission setup: Photons with the energy hν impinge on the sample surface and excite electrons. The emitted photoelectrons are focused intoa hemispherical analyzer. The kinetic energy as well as the emission angle will be measured.The emission angle is varied by turning the sample around θ and Φ and the third direction iscovered by the acceptance angle of the analyzer. After passing the analyzer the electrons aredetected with a 2D CCD camera.
27
Chapter 3. Experimental Techniques
of the primary spectrum [107]. When analyzing EDCs one has to consider also the cuto
at the Fermi level due to the change in occupation of the electronic states. For the tting
procedure of the remaining primary spectrum peaks with a Voigt line shape, a convolution
of Lorentzian and Gaussian functions, are used. The complete tting function for an EDC
is given by:
I(E) = c+BS(E) +
[∑i
L(E,Ei,Γi) ∗G(Γres)
]f(E − EF , T )
The constant oset c accounts for the dark count rate in the detector. L(E,Ei,Γi) are the
Lorentzians [see Eq. 3.3] with the peak positions at Ei and the full width at half maximum
Γi = 2Im(Σ) that describe the single peaks. The Gaussian function G(Γres) accounts for
the experimental resolution Γres.
The measurements presented in Chap. 4 and 5 have been carried out at the Max
Planck Institute for Solid State Research (MPIFKF) in Stuttgart. A hemispherical SPECS
electron analyzer (energy and angular resolution are 15meV and 0.5, respectively) and
a monochromatized He lamp that oers UV radiation at hν = 21.2 eV (He I) and hν =
40.8 eV (He II) are attached to the UHV chamber with a base pressure p = 2 · 10−10 mbar.
The manipulator can be cooled with liquid nitrogen to about −180 C.
The ARPES experiments shown in Chap. 6 have been performed at the University of
British Columbia in Vancouver. The UHV chamber is equipped with a SPECS Phoibos
150 hemispherical analyzer and a UVS300 monochromatized gas discharge lamp. Energy
and angular resolution were set to 15meV and 0.3. Linearly polarized photons with an
energy of 40.8 eV were used. During ARPES measurements the samples were kept at 8K
at a pressure less than 7 · 10−11 mbar.
The data shown in Chap. 7 were taken at the Synchrotron Radiation Center (SRC)
in Stoughton, Wisconsin, USA at the variable polarization VLSPGM beamline. This
beamline was equipped with an elliptically polarized Apple II undulator that delivers p
and spolarization of photons in an energy range from 15 eV to 250 eV. A Scienta analyzer
with an energy resolution of about 10meV and an angular resolution of 0.4 has been used.
The manipulator could be cooled with liquid helium down to 30K. The base pressure of
the UHV chamber was p = 1 · 10−10 mbar.
28
3.3. Core level spectroscopy
3.3 Core level spectroscopy
Core level spectroscopy, also known as Xray photoemission spectroscopy (XPS) is a pow
erful tool to study the chemical composition or to determine the binding energies of the
atomic core levels of elements in a solid [113]. A photon source that delivers photons in the
soft Xray region is needed to provide enough energy for excitation of core electrons. The
binding energy of the core levels is determined by measuring Ekin of the photoelectrons for
normal emission and using Eq. 3.1. A schematic illustration of the photoemission process
in XPS is drawn in Fig. 3.1.
Since every element has a characteristic series of binding energies for its core electrons
XPS serves to determine the chemical composition of the sample surface by comparing the
measured peak positions to reference spectra. For precise identication one can additionally
check the intensity ratio and separation of some spin doublets for p, d and f lines. Due
to SOC all core levels with nonzero angular momentum (l 6= 0) are split into branches.
Furthermore the holes created in the atoms give rise to the emission of socalled Auger
electrons, which can be detected in the spectrum too.
When elements are mixed in compounds, the binding energy of the peak under inves
tigation shifts slightly by an amount ∆EB, which is called the chemical shift. Whether
this shift is positive or negative is determined by the eective electronic potential variation
induced by the charge distribution between the elements forming the compound. Further
more, the shift depends on the bonding type, on the electronegativity of the elements, and
on the interaction between the photoionized atom and the rest of the crystal [107]. By
measuring the small shifts one can use XPS to determine the chemical state of an atom.
This is the reason why formerly XPS was also called ESCA which stands for electron
spectroscopy for chemical analysis.
It is also possible to analyze XPS spectra quantitatively. The integrated intensity of
the peaks give access to the concentration of a particular material. One has to take care
about the secondary electrons. The main peaks in the photoemission spectrum correspond
to electrons that leave the surface without energy loss. Electrons that undergo inelastic
scattering events contribute to the Shirley background.
All core level spectra shown in this thesis were measured at the MPIFKF in Stuttgart.
The measurements have been performed at room temperature using nonmonochromatized
Mg Kα radiation at hν = 1253.6 eV. The spot size of a conventional Xray source is about
a few mm2. XPS has been used mainly to check the cleanliness of the substrate.
29
Chapter 3. Experimental Techniques
30
Chapter 4
Coulomb interaction in topological
insulators
A 3D TI is a quantum state of matter characterized by an insulating bulk state and gapless
surface states that show a peculiar spin texture [see Sec. 2.2.2]. Possible applications of TIs
in electronic devices require a highly insulating bulk and tunable Dirac carriers. Due to the
coexistence of both bulk and surface conduction in Bi2Se3, it is dicult to investigate the
topological properties separately. In ongoing research, there are extensive eorts to reduce
bulk carriers in Bi2Se3 through material doping [41,51,114], nanostructuring [57,115,116]
and electric gating [117,118]. By replacing Se with Te atoms, the bulk insulating property
could be considerably improved. Accordingly, Bi2Te2Se is a system where the energy gap
is ∆ ≈ 0.3 eV and the chemical potential is located within the bulk band gap [119].
Common theoretical descriptions of TIs are formulated in terms of singleparticle quan
tum mechanics. Due to quite large lattice dielectric constants (> 50) in TIs and the very
small corresponding eective ne structure constant, it is often claimed that electron
electron interactions are negligible and does not alter the topological properties [59]. But
it was shown that the electronelectron interaction is often needed to describe experimental
observations [120122]. If the interaction is very strong it can even turn the topological
phase into an insulating ground state [6] or induce a novel critical state on the surface [123].
Therefore, it is a crucial issue to understand the interplay between strong electronelectron
interaction and the topological surface states [124,125].
31
Chapter 4. Coulomb interaction in topological insulators
4.1 Bi2Se3, Bi2Te3 and Bi2Te2Se
The 3D TIs Bi2Se3 and Bi2Te3 and also the mixture Bi2Te2Se have a tetradymite structure.
All materials of this family crystallize in covalently bonded QLs weakly interacting via van
der Waals force [5]. As shown in Fig. 4.1(a) the stacking order is ABCABC. Each
quintuple layer is about 1 nm thick and the lattice constant along the caxis is about 3 nm.
TeBiSe
Bi
Te
Bi
TeSe
(a)
unit
cel
l
(b)
Figure 4.1: Crystal structure of tetradymite chalcogenides, using the example of Bi2Te2Seand the corresponding surface band structure. (a) QL enclosed by the brown cage is thebuilding block of this type of materials. The stacking order of the QLs is ABCABC, andhence the unit cell consists of a stack of 3 QLs. (b) Topological surface state measured withARPES.
The interesting properties of those materials are connected to their electronic structure
and, particularly, the low energy region. The states close to the Fermi energy are mainly p
orbitals. Therefore, the opposite parities originate from bonding and antibonding states.
By taking into account chemical bonding, crystal eld splitting and SOC, a pair of inverted
energy bands is found at the Fermi level. This inversion drives the system into a TI
phase. The bulk insulating gap is ∆ ≈ 0.3 eV, which results in the possibility of having
a topological phase at room temperature. To describe the lowenergy properties of those
systems an eective Dirac model is used.
Due to naturally occurring crystalline defects in Bi2Se3 and Bi2Te3, their bulk is always
highly doped and their transport properties are always dominated by bulk carriers. The
32
4.2. Doping behavior
key for the preparation of a TI with large bulk resistivity is to shift the Fermi level into
the bulk band gap. For example, by mixing Te and Se atoms, Bi2Te2Se can be fabricated,
in which the chemical potential is located between valence and conduction band of the
bulk and which shows a large bulk resistivity exceeding 1Ωcm [119]. By this shift of the
chemical potential the contribution from the surface states to the conducting electrons is
strongly enhanced. It is the rst 3D TI where detailed transport studies of the topological
surface state are possible. Clear Shubnikovde Haas oscillations are observed and they
contribute ∼ 6% to the total conductance in a 260µmthick bulk crystal. Xiong and
coworkers reported an even larger resistivity of 6Ωcm [126].
For the investigation of the surface state band structure including manybody eects in
3D TIs ARPES is the technique of choice. ARPES probes directly the 2D band structure
which contains all the manybody phenomena [see Chap. 3.1.2]. Bi2Te2Se crystals were
grown in the group of Prof. Claudia Felser at the MPICPfS in Dresden. The samples were
glued to a sample holder and cleaved in vacuum via mechanical exfoliation. As a photon
source, the HeI line was used. In Fig. 4.1(b) the band structure of a freshly cleaved surface
is presented. This measurement and all subsequent ones on this system were performed at
room temperature. The topological surface state in the bulk band gap is clearly visible. The
Dirac point almost coincides with the top of the valence band at around EB = 0.2 eV. From
the Fermi level down to this point we only see the Dirac cone and a very low background.
There are only the topological states at the Fermi level and for them back scattering is
forbidden. Hence, the bands are quite sharp and they are almost linear dispersing. We
note that there is no sign of the conduction band visible at the Fermi level and that the
resulting bulk band gap is quite big. All our experimental ndings coincide with previous
ARPES measurements [55].
4.2 Doping behavior
If the freshly cleaved sample is left in the UHV chamber for some time, a shift of the Dirac
point to higher binding energies can be observed. This timedependent doping eect can
be explained by contamination of the surface from residual gas in UHV. The adsorbates
give rise to a strong band bending of the bands near the surface. A similar eect was also
observed for Bi2Se3 [127, 128]. In Fig. 4.2 the band structure measured at dierent delay
times with respect to the cleavage procedure is shown.
The small black arrows indicate the position of the Dirac point, which shifts to higher
33
Chapter 4. Coulomb interaction in topological insulators
0.1 0 0.1
k (Å1
)
0.1 0 0.1
k (Å1
)
0.1 0 0.1
k (Å1
)
0.8
0.6
0.4
0.2
0.0
0.2In
itial
Sta
te E
nerg
y (e
V)
0.1 0 0.1
k (Å1
)
0 h 25 h18 h1 h
Figure 4.2: Timedependent doping of the topological surface state at Γ in Bi2Te2Se whileresting in vacuum. Dirac point shifts to higher binding energy over time as indicated by theblack arrows. The duration between cleave and measurement is indicated in the upper rightcorner of the panels.
binding energy over time. After 25 hours the total shift of the Dirac point amounts 170meV.
Despite the large shift, we still do not see any indication from the conduction band at the
Fermi level. Hence, we conclude that the gap is at least ∆ = 0.37 eV. Due to the band
bending, the charge carrier density n increases. We determined the Fermi wave vector kFand extracted n. Both are graphically shown in Fig. 4.3.
Both kF and the corresponding n increase over time. Since we have only four data
points we can just surmise that in the beginning the band bending goes almost linearly
whereas it starts to saturate after 18 hours. During roughly one day in UHV the charge
carrier density increases by the factor of 2.8 due to adsorption of residual gas molecules.
This gives us the opportunity to study the eect of dierent charge carrier densities on the
strength of manybody interactions in TIs.
4.3 Coulomb interaction at low charge carrier densities
The images in Fig. 4.2 show clearly the shift of the surface states to higher binding energies
(as indicated by the small arrows) and the increase of the Fermi wave vector kF over time.
To evaluate the manybody physics in the system we had a closer look at the linewidth,
since it is proportional to the imaginary part of the selfenergy. In the following analysis
we stick to the extreme cases  the freshly cleaved, clean sample and the one that remained
for 25 hours in vacuum (now called the 'aged sample'). We took the single MDCs and
34
4.3. Coulomb interaction at low charge carrier densities
0.12
0.11
0.10
0.09
0.08
0.07
0.06
Ferm
i wav
e ve
ctor
(Å
1)
2520151050hours after cleave
14
12
10
8
6
4
2
0
charge carrier density (1012cm
2)
Figure 4.3: Timedependent increase of the Fermi wave vector kF as well as the chargecarrier density n in Bi2Te2Se.
tted them as exemplarily shown in Fig. 4.4(a). Presumably, an imperfect alignment
of the sample leads to a dierence in linewidth of the left and the right branch and we
determined them separately. The extracted linewidth from every single peak of the left
branch as a function of binding energy for the clean and the aged sample is plotted in Fig.
4.4(b).
For both the clean and the aged sample the linewidth has a minimal value at the Fermi
level and increases with increasing binding energy. We also notice that the absolute value
of the linewidth at the Fermi level is larger for the aged sample. This can be explained
by the adsorbed gas molecules, which induce disorder at the surface leading to a constant
oset in the linewidth. In fact, the linewidth for the aged sample is larger at the Fermi
level, but the increase of the linewidth is smaller.
As introduced in Sec. 3.1.2 there are two energy dependent scattering mechanisms
that can contribute to broadening of the linewidth; electronelectron and electronphonon
interaction. The Debye temperature TD in Bi2Te2Se is assumed to be comparable to the
one in Bi2Se3, which is TD = 182K (∼ 16meV) [129]. Since our measurements were
performed at room temperature the thermal energy is above TD and we do not expect
an energy dependent contribution due to interaction with phonons. Therefore, we instead
attribute the energy dependent increase of the linewidth to electronelectron interactions.
The dierence in the increase of the linewidth can be explained by varying screening
35
Chapter 4. Coulomb interaction in topological insulators
Inte
nsity
(ar
b. u
nits
)
0.10 0.00 0.10
Momentum (Å1
)
(a) (b)
0.04
0.03
0.02
linew
idth
(Å
1)
0.10 0.00EEF (eV)
aged clean
left branch
Figure 4.4: (a) Exemplary t of two Lorentzian to a MDC cut through the topologicalsurface state. (b) Increase of the linewidth as a function of energy for two dierent dopinglevels.
strength due to the dierence in the total number of charge carriers. The only dierence
between the two samples is the charge carrier concentration at the Fermi level. Due to
doping, i.e. the shift to higher binding energies, and the linear dispersion the Fermi surface
volume increases over time, which results in a higher charge carrier density at zero binding
energy. The more electrons are available, the higher the screening of the interaction. If
the interaction is eciently screened the linewidth broadening due to electronelectron
interactions is reduced.
In addition to the change in linewidth, we observe a change of the Fermi velocity, i.e.
the slope of the bands at the Fermi level, over time [see Fig. 4.5]. We noticed that the
band velocity at the Fermi level is bigger for the aged sample. This can be explained by a
renormalization of the Fermi velocity due to the electronelectron interaction, which results
in a band that disperses less steep compared to the noninteracting case. Since the number
of charge carriers increases by going from the clean to the aged sample, the eciency of
the screening rises and hence, the band velocity increases over time.
For more quantitative statements about linewidth and band velocity, we compare the
results of the MDC ts to a theoretical model. With data sets at dierent doping levels and
by considering selfconsistency we are able to determine the parameters for the complex
selfenergy and the bare band dispersion. We performed model calculations in 2D for the
36
4.3. Coulomb interaction at low charge carrier densities
0.12
0.08
0.04
0.00
EE
F (
eV)
0.10 0.05 0.00 0.05 0.10
Momentum (Å1
)
bare dispersion 0h 25h
(shifted by 0.175eV)
Figure 4.5: Comparison of the band dispersion close to the Fermi energy. To be able tocompare the slopes, the band structure of the aged sample was shifted by 0.175 eV to smallerbinding energies. For the freshly cleaved sample we observe the smallest slope, since screeningis not sucient due to the small number of charge carriers.
spectral function [see Eq. 3.3] by assuming a bare band dispersion of the form
E0~k
= vF ~k+ ε0 (4.1)
Since we attribute the increase of the linewidth and the Fermi velocity to electron
electron interactions we assume a quadratic energy dependence (ImΣ(ω) ∝ ω2, see Eq.
3.4) for the imaginary part of the selfenergy [130]. The imaginary and the real part of
the complex selfenergy are connected via a Hilbert transformation H: ReΣ = H(ImΣ).
Therefore, we choose for the selfenergy the following ansatz:
Σ(ω) = i(β1ω2 + α)− β2ω (4.2)
The parameter α serves as a constant oset in the linewidth, while β1 forms the real
part and β2 is the coupling constant for electronelectron interaction. For reasons of self
consistency, the ratio between the coecients will be held constant β1/β2 = const. for
all doping levels. In our case the ratio was found to be β1/β2 = 2. We note that the
band velocity of the bare dispersion is also xed for all doping levels. We calculated the
spectral function [Eq. 3.3] using the bare dispersion in Eq. 4.1 and the selfenergy from
Eq. 4.2. After a convolution of the band structure with a Gaussian to account for the
37
Chapter 4. Coulomb interaction in topological insulators
experimental momentum and energy resolution the calculated MCDs were tted with two
peaks of Lorentzian shape. We compared the calculated values for peak position and
linewidth to the experimental ones by applying a χ2test. The smallest value for χ2 tells us
the best tting values for the three parameters. With this procedure we are able to handle
both data sets at dierent doping levels at the same time. We found a set of parameters
that matches the position and hence the slope of the bands as well as the linewidth of the
peaks for the clean as well as for the aged sample. The t results for the experimental
and the theoretical peak positions are presented in Fig. 4.6(a). The calculated linewidths
are shown together with the experimental ones in Fig. 4.6(b). For the model calculations
we also treated the two branches separately. All important t parameters are collected in
Table 4.1.
ε0 (eV) vF (eVÅ) β1 (1/eV) β2 n (1012 cm−2)clean (0h) 0.3 4.5 0.62 0.31 3.5aged (25h) 0.51 4.5 0.18 0.09 10.2
Table 4.1: Results of the χ2test for the parameters of the bare band dispersion [Eq. 4.1]and the complex selfenergy Σ [Eq. 4.2]: energy oset of the Dirac point ε0, Fermi velocity inthe bare band dispersion vF , electronelectron interaction constant β1, the parameter for thereal part of Σ β2; for comparison: charge carrier density n.
In addition, our model combined with data sets at dierent doping levels and the χ2test
allows us to extract the band velocity of the bare dispersion. With ARPES we measure the
real band structure, which is the result of the combination of the noninteracting system
plus interactions. Solely because we have two data sets which we can compare and handle
selfconsistently we are able to determine the band dispersion without interaction. We
found a bare band velocity of 4.5 eVÅ. In order to compare it to the renormalized bands
we plotted it in Fig. 4.5.
4.4 Discussion
Looking at the t results we see, that the rst value, which we determined, is the energy
shift of the band structure ε0. As we see in Fig. 4.2 the cone shifts to higher binding
energy over time and we expect a larger shift for the aged sample. Indeed we nd a ε0whose absolute value is larger for the aged sample. The dierence between clean and aged
sample is 210meV which is in the order of the experimental observed shift of 170meV.
The deviation of 40meV can be explained by the band renormalization. For the coupling
38
4.4. Discussion
0.20 0.15 0.10 0.05 0.00EEF (eV)
exp. width left exp. width right calc. width
aged
0.04
0.03
0.02
linew
idth
(Å
1)
0.10 0.05 0.00EEF (eV)
exp. width left exp. width right calc. width
clean
0.120.080.040.00
EE
F (
eV)
0.10 0.05 0 0.05
Momentum (Å1
)
0.25
0.20
0.15
0.10
0.05
0.00
0.10 0 0.10Momentum (Å
1)
experimental peak position calculated peak position
agedclean(a)
(b)
Figure 4.6: Comparison of experimental and calculated peak positions as well as linewidthsfor the topological surface state in Bi2Te2Se. The experimental values were found by ttingtwo Lorentzians to every MDC. The theoretical values were determined by calculating thespectral function with the complex selfenergy from Eq. 4.2 and performing the same tprocedure as for the data. Note that left and right bands are treated separately.
39
Chapter 4. Coulomb interaction in topological insulators
constant β1 and since the ratio is constant also for β2 we nd that it is a factor of 3
larger for the clean sample. By keeping the sample one day in vacuum the electronelectron
interaction diminishes to 30% of the starting value. This tells us that the interaction in the
freshly cleaved sample is much higher than in the aged one. If we compare the charge carrier
densities of the two samples which can be found in the last column of Table 4.1 we also nd
roughly a ratio of 3 for clean and aged sample. This fact supports our assumption that the
electronelectron interaction increases if n is getting smaller and leads us to the conclusion
that β1 is inverse proportional to n. Beside n, the dielectric constant ε determines the
strength of the screening. Since we measured all data on the same sample we assume the
same ε.
A much smaller value for ε applies for graphene. This is the reason, why the quasipar
ticle dynamics was studied intensively for graphene. The dielectric constant in graphene
is about 10 times smaller than of TIs. For small values of ε, screening is not sucient
and the Coulomb interaction is stronger. The eect of the charge carrier density on the
other hand is negligible in graphene. The charge carrier densities which we observe usually
in our graphene samples [see Chap. 6] are comparable to the ones in the aged Bi2Te2Se
sample. There should be enough charge carriers available to screen the electronelectron
interaction. Nevertheless, the small ε in graphene leads to a substantial renormalization of
the band structure.
For a more quantitative conclusion in the case of Bi2Te2Se it would be desirable to nd
a way to connect the parameters β1 and β2 or their ratio to the strength of the screening.
We would expect that the parameter β1 shows the following dependency: β1 ∼ 1/(εn).
Therefore, more detailed measurements and theoretical considerations are necessary.
Our analysis procedure in this chapter can be transferred to many other studies of many
body physics with ARPES. We have shown how to handle electronelectron interaction but
one could think of applying our analysis procedure also on electronphonon interaction. The
ingredients for a detailed analysis are a formula for the selfenergy and a proper ansatz for
the bare band dispersion. As long as only one data set is available the model is able to
nd the parameters for Σ. Selfconsistency helps to determine both the real part as well
as the imaginary part [131]. But for an advantageous situation like ours when there are
measurements done at dierent n the model allows even for a determination of the bare
band dispersion. In a more general sense we have used the measured and the calculated
spectral function to nd the complex selfenergy in Bi2Te2Se.
In summary, electronelectron interactions are usually neglected in TIs since the dielec
40
4.4. Discussion
tric constant ε is quite large. However, we observe a substantial band renormalization of
the surface states in Bi2Te2Se dependent on the charge carrier density and on the binding
energy. Due to time dependent doping caused by the adsorbed molecules from the residual
gas in UHV we are able to investigate the band renormalization for dierent doping levels.
Combining the data sets allows us to determine the parameters for the complex selfenergy
selfconsistently and to extract the contribution from electronelectron interactions to the
linewidth broadening. Additionally, we found also a value for the band velocity without
interactions. We conrm that electronelectron interactions or more general, manybody
physics is necessary to describe all the properties of topological surface states.
41
Chapter 4. Coulomb interaction in topological insulators
42
Chapter 5
Surface band structure of TiTe1.5Se0.5
In addition to the careful investigation of the already known TIs, it is also very important
to look for new materials with topological states and peculiar properties. The rst ex
perimentally conrmed TIs HgTe [42] thin lms and Bi1−xSbx [38] are quite dicult
to fabricate and show a complex surface band structure, respectively. However, with the
discovery of bismuth compounds with topological properties, it was shown that topologi
cal surface states can also be found on inexpensive and readily available materials. This
opened the door for a very intensive research eld in which scientists are looking for new
topological materials [132].
5.1 Search for new topological materials
The motivation for nding new topological materials is twofold; on one side it is interesting
for fundamental research and on the other side it is very important for the development of
electronic devices containing TIs. In the rst case, the driving force is to discover and study
new physical phenomena. One goal is to achieve a better understanding about what turns
a material into a TI. For applications of TIs, scientists are also interested in nding new
topological materials that have some practical advantages compared to the known ones.
They are looking for TIs that are, for example, easier to fabricate, which have higher bulk
resistivity or TIs in which the charge carrier density can be easily tuned. Several families
of 2D and 3D TIs have been proposed theoretically and have been, in part, conrmed
experimentally [see Sec. 2.2.2].
For a systematic approach for nding new ones, we have to combine all the experimental
results with the established theoretical knowledge and attempt to make strong predictions.
43
Chapter 5. Surface band structure of TiTe1.5Se0.5
In particular, it is important to consider the band structure considering its crucial role.
For example, ab initio calculations can help to establish a topological phase diagram and
to search for nontrivial surface states [133]. For example, in TiS2−2xTe2x a topological
nontrivial phase was predicted for 0.48 < x < 0.80 in 2D as well as in 3D.
Since SOC is often responsible for the required band inversion of the topological state
a promising approach is to look for systems with narrow band gaps and heavy atoms.
Many new topological materials consist of elements from the lower right corner of the
periodic table. Examples are Bi [39], Pb [134] and Tl [49] based chalcogenides. In addition,
mixing of element compositions has proven successful. With these points in mind, titanium
dichalcogenides are also promising candidates.
5.2 Crystal structure
In general, transition metal dichalcogenides (TMDCs) have been attracting attention for
more than 40 years due to their diverse properties [135, 136]. For example, electrically
they cover the whole spectrum from insulators (HfS2) through semiconductors like MoS2,
to semimetals (WTe2) and true metals like NbS2. The properties of some of the TMDCs
can be tune via a structural distortion. Even superconductivity, charge density waves and
antiferromagnetism were observed in TMDCs [135,137].
Se/Te
Ti
Figure 5.1: Crystal structure of TiX2. Every chalcogenide (green) atom is bound to threetitanium (red) atoms. The van der Waals gap lies inbetween the chalcogenide layers. Thedepicted cube illustrates the unit cell of the structure.
Like all TMDCs, the ones with Ti consist of XTiX (X= S, Se, Te) composite layers.
They are stacked like the layers in graphite and bound by weak van der Waals interactions
44
5.3. Electronic structure
acting perpendicular to the sheets. Those compounds crystallize in the 1T CdI2 prototype
structure [138]. Such layered structures show typical quasi2D behavior. The unit cell
is depicted in Fig. 5.1. If the chalcogenides are exchanged or mixed, no structural phase
transition is expected as the lattice parameters are adapted. The lattice constants for
TiSe2 are a = 3.540Å and c = 6.008Å, for TiTe2 they are a = 3.777Å and c = 6.498Å
and for the mixture TiTeSe a = 3.651Å and c = 6.317Å were found [138].
TiSe2 was intensively studied because of the occurring charge density wave at low tem
peratures. On the other hand, those materials are known for their intercalated derivatives
like in the case of TiS2. Foreign atoms can easily be introduced into TMDCs at the van der
Waals gap and can modify the properties of the compound radically. Those intercalated
compounds have been employed as a cathode material in rechargeable batteries, but they
can also be used as strongly anisotropic conductors and ordered magnetic systems [139].
5.3 Electronic structure
The electronic band structure of monolayer TiS2 and TiTe2 in the presence of SOC was
calculated in [133] and is shown in Fig. 5.2. The authors predict a topological nontrivial
state for TiS2−2xTe2x from 0.48 < x < 0.80.
Figure 5.2: Electronic band structures of monolayer (a) TiS2 and (b) TiTe2, in the presenceof SOC. The dierent colors indicate the band characters as the bar on top shows. (c) and (d)show a zoomin at the Γpoint and the band hierarchy. Symmetry is labeled, and even/oddparity is indicated by +/ (taken from [133])
45
Chapter 5. Surface band structure of TiTe1.5Se0.5
In this case we can exemplarily follow the band inversion by going from TiS2 to TiTe2.
For both materials, the bands with S/Te p character are lled whereas the Ti d bands
are almost empty. In the lower panels of Fig. 5.2 the parity of the states is indicated.
In TiS2 the odd parity states are separated from the even parity states by EF and the
material turns out to be an indirect band gap semiconductor. The valence band maximum
is located at the Γpoint and the conduction band minimum at the Mpoint for both
materials. However, in the case of TiTe2 the states are entangled and the energy band gap
is lost. At the Γpoint the bands are inverted but the material is still topologically trivial.
However, by mixing S and Te the material can be turned into a TI.
Since all the chalcogen atoms are isoelectronic, Se has the same number of electrons in
the outer shell but one shell more than S and one shell less compared to Te. By replacing S
with Se, SOC is slightly increased. Accordingly, the surface band structure of the mixture,
TiTe2xSe2−2x, should be comparable to the one of TiTe2. To check if these assumptions
are true we performed ARPES measurements of TiTe1.5Se0.5 crystals where x = 0.75.
The crystals were grown in the group of Prof. Lotsch at the MPIFKF in Stuttgart.
After inserting them into the UHV chamber they were mechanically cleaved in situ. Before
the ARPES measurements we checked the properties of the surface. The XPS overview
spectrum in Fig. 5.3 shows several peaks that we identied through comparison to literature
[113].
(a) (b)
Figure 5.3: Surface analysis of TiTe1.5Se0.5: (a) XPS and (b) LEED at E=51 eV.
In addition to all expected elements (Ti, Te, Se) we found peaks for Ag, O and C. The
small Ag peaks originate from the glue used to x the sample on the sample holder. Since
the crystals are very small it was impossible to eliminate the Ag peaks. Appearance of
oxygen and carbon can be explained by the growing process and transportation through
46
5.3. Electronic structure
air before inserting into UHV. However, the intensity of the C and O peaks is quite small
and thus they can be neglected. Overall, XPS conrms that the crystal surface is clean
enough for ARPES measurements. To check the structural properties of the surface we
did also LEED measurements at 51 eV and observed a clear hexagonal structure [inset in
Fig. 5.3].
0.2 0.0 0.2
ky (Å1
)
0.2 0.0 0.2
ky (Å1
)
1.2
0.8
0.4
0.0
Initi
al S
tate
Ene
rgy
(eV
)
0.2 0.0 0.2
ky (Å1
)
1.5
1.0
0.5
0.0
Initi
al S
tate
Ene
rgy
(eV
)
1.00.50.00.5
Wave Vector kx (Å1
)
Γ M
kx=0 Å1
kx=0.4 Å1
kx=0.8 Å1
Figure 5.4: Surface band structure of TiTe1.5Se0.5 in ΓM direction. In the lower panels cutsperpendicular to ΓM at indicated positions are shown.
In Fig. 5.4 the measured surface band structure of TiTe1.5Se0.5 at room temperature
is shown. We compare our experimental results to the calculated band structure of TiTe2
and observe many similar structures. There are two bands above the Fermi level that
build a hole pocket at the Γpoint [see lower left panel of Fig. 5.4]. In ΓMdirection they
disperse downwards and cut the Fermi level at about kx = 0.12Å −1. At kx = 0.4Å −1 we
47
Chapter 5. Surface band structure of TiTe1.5Se0.5
can clearly distinguish two bands in the panel in the middle. The second clear feature is a
small electron pocket at the Mpoint with the band minimum at E = 0.3 eV. In the lower
right panel of Fig. 5.4 the electron pocket at k = 0.8Å −1 perpendicular to the ΓMdirection
is shown.
To judge whether TiTe1.5Se0.5 is a topological nontrivial material we would need to see
the inverted band gap and to measure a topological surface state. However, it was so far
impossible to observe the band gap because it lies in the unoccupied states at the Γpoint
as can be assumed by looking at Fig. 5.2(d). With ARPES we are able to study only
the occupied states. For the observation of a possible topologically protected surface state
sucient electron doping would be needed to shift the band gap below the Fermi level.
5.4 Discussion
Our experiments are just the rst step of identifying TiTe1.5Se0.5 as a TI. So far, it appears
to be a promising candidate and further investigations are desirable. There are also many
other proposals for TMDCs as 2D quantum spin Hall insulators. Especially for MX2 with
M=(Mo, W) and X = (S, Se, Te) a lot of theoretical studies are done and unique properties
are predicted [140, 141]. Those 2D materials are fascinating because of their similarity to
graphene and the possibility to build 2D heterostructures by stacking dierent 2D sheets
on top of each another [142]. So far, those van der Waalsheterostructures have not been
considered for topological phases of matter [132, 143]. Therefore, we see a new research
eld developing and expanding in the near future.
In addition to their topological properties, TMDC nanostructures have attracted in
creasing attention because of their versatile chemical properties in contrast to graphene.
Monolayers of TMDCs are usually semiconductors with varying band gaps and variable
charge carriers (n or ptype). By changing their composition, their structure or their di
mensionality, these materials can be very attractive for a variety of applications [144146].
For example, many of the TMDCs show layer dependent behavior. For example, several
semiconducting TMDCs undergo a transition from an indirect gap in the bulk to a direct
bandgap for a monolayer [147]. The direct bandgap in the monolayer is usually larger than
in the bulk and opens the possibility of many optoelectronic applications [146].
TMDCs are also very promising candidates for photocatalytic water splitting. In
particular, monolayers of metal disuldes show very good catalytic performance in water
splitting [148]. The electrolysis of water driven by catalysts is considered as the 'cleanest'
48
5.4. Discussion
way for hydrogen production. One major goal in the research eld of hydrogen production
is to nd cheap and abundant catalysts that are suitable for largescale implementation in
technology. Other interesting applications are in the eld of energy storage as electrodes
in Liion batteries or as photovoltaics [149].
Due to the lack of an inversion center in the crystal structure of TMDC monolayers
a new degree of freedom of the charge carriers is accessible: the valley index. Taking
advantage of this fact is the main goal of valleytronics, a new eld of physics [150,151].
49
Chapter 5. Surface band structure of TiTe1.5Se0.5
50
Chapter 6
Scattering mechanisms in thallium
doped epitaxial graphene
Due to its unique and very interesting properties graphene is a promising candidate for
future generations of extraordinarily fast electronic devices. The electron mobility at room
temperature, which is higher than in any other known material, results from the funda
mental symmetry and the strict twodimensionality of the graphene honeycomb lattice. If
the perfect symmetry is broken by either a defect or an impurity the electrical properties
can be changed substantially. In many cases, this can be actually advantageous and some
properties can be even improved by the appropriate introduction of impurities. Examples
are chargetransfer doping through adatoms or molecules to tune the position of the Dirac
point with respect to the Fermi level [152156], and also dierent interactions (electron
electron or electronphonon) [98, 157, 158], metalinsulator transitions [159, 160] and so
far only at the level of theoretical prediction the emergence of superconductivity [161]
or of topologically insulating behavior [162].
On the other hand, defects or impurities in the graphene lattice can also disturb or
damage the electronic properties. Every time impurities are introduced they give rise
to unavoidable mobilitylimiting disorder and enhanced scattering [163]. Ecient doping
by molecules even necessitates the presence of defects in the graphene layer [164]. In
most cases, adatoms reduce the quasiparticle lifetime by introducing longrange (Coulomb)
scattering and/or shortrange (δpotential) scattering. The latter has been proposed to be
largely responsible for graphene's residual conductivity [163]. In order to gain more insight
into the electronic properties of graphene, it is important to analyze and understand how
51
Chapter 6. Scattering mechanisms in thallium doped epitaxial graphene
impurities aect them.1
6.1 Impurities on graphene
There are several dierent ways for an impurity to connect itself to graphene. This ranges
from weaklyattached physisorption [165] to the formation of a covalent bond as in the
example of hydrogen, which sp3hybridizes the carbon bond [159]. The impurity can also
donate charge to the graphene layer and act as a charged impurity. In any case, graphene's
electronic structure will be aected somehow.
In general, the charge carrier mobility µ is inversely proportional to the density of
charged impurities nimp. This translates into an increase of the scattering rate upon doping.
There are also other reports that claim an increase of the quasiparticle lifetime upon doping
with charged impurities [166]. Such behavior critically depends on screening, which is
determined through the dielectric constant ε of the system. Depending on ε, dierent
scattering mechanisms can become more pronounced or suppressed. Coulomb scattering
is often assumed to be the dominant scattering mechanism in graphene, but shortrange
scattering can become appreciable if dielectric screening is highly eective in reducing
Coulomb scattering.
Impurities with states close to the Fermi level also give rise to a particularly strong
scattering potential [167]. In this sense, shortrange scattering can also be present for
noncovalently bonded impurities. Therefore, in real systems, it is not necessarily a priori
clear which scattering mechanism is dominant. With ARPES measurements it is possible
to observe the scattering behavior induced by Tl adatoms on graphene and disentangle
longrange from shortrange scattering contributions.
Tl atoms on graphene is a particularly interesting model system as it nicely demon
strates the diculty in predicting the scattering behavior beforehand. We show that it
features a sizeable shortrange scattering contribution even though its adsorption behavior
is similar to potassium; it is extremely weakly bonded to graphene and highly mobile at
temperatures above 15K. Only by employing the electronic structure of the unperturbed
Tl atom, we are able to theoretically predict the scattering behavior. In addition, Tl has
been proposed as one of the most promising candidates to open a SOC related gap at the
Dirac point turning graphene into a TI [162].
Epitaxial graphene monolayers with a buer layer were grown under Ar atmosphere on
1The present chapter is based on publication 3 from the list attached at the end of this thesis.
52
6.2. Doping eect of Tl adatoms
hydrogen etched 6HSiC(0001) at the MPIFKF in Stuttgart. To remove the adsorbed gas
molecules from air, the graphene samples were postannealed at 700C after insertion into
UHV in the ARPES chamber in Vancouver. It has been calculated that Tl is one of the
most mobile atoms on the graphene surface [168]. Therefore, Tl atoms were evaporated
from an electron beam evaporator on a cold sample at 8K to avoid surface diusion and
clustering. All subsequent measurements were done at similar temperatures.
6.2 Doping eect of Tl adatoms
Fig. 6.1 shows the experimentally determined band structure of an epitaxial graphene
monolayer near the Kpoint as a function of Tl coverage.
Momentum (Å1
)0.1 0 0.10.1 0 0.10.1 0 0.10.1 0 0.10.1 0 0.1
1.0
0.8
0.6
0.4
0.2
0.0
E 
EF (
eV)
0.1 0 0.1
0.0% 0.5% 0.8% 1.0% 2.3% 3.3%
Figure 6.1: Monolayer graphene decorated with small amounts of Tl atoms. Experimentalband structure near the Kpoint for increasing Tl concentration x measured at 8K with aphoton energy of 40.8 eV.
The concentration x of Tl atoms on the surface is given in percent of a graphene
monolayer, i. e. the number of Tl atoms per carbon atom. The lefthand side data set
is from the pristine graphene monolayer, exhibiting an initial ntype doping due to the
intrinsic charge transfer from the SiC substrate. Upon Tl deposition, electron doping
increases so that the Dirac point shifts to higher binding energies, away from the Fermi
level. We attribute this to charge transfer from the Tl atoms to the graphene. The largest
energy shift we observed was ∆E ≈ 0.2 eV. For concentrations higher than 1%, the trend
is reversed, and the Dirac point shifts back towards the Fermi level. We ascribe this to
the statistical eect that for concentrations higher than about 1% pairing and clustering of
atoms become nonnegligible, which reduces the eciency of charge transfer doping [169].
53
Chapter 6. Scattering mechanisms in thallium doped epitaxial graphene
This statement is conrmed by temperature dependent measurements, where we ob
serve and conrm that Tl atoms are extremely mobile on the graphene surface at higher
temperatures (cf. [168]). This is illustrated in the temperature dependence of the relative
energy shift of the Dirac point in Fig. 6.2(a) for a Tl coverage of 0.5%. Above 15K, a rapid
decrease in doping eciency can be observed, which we attribute to clustering of Tl atoms.
We conclude that Tl is only very weakly and not covalently bonded to the graphene and
thus migration barriers are very small. For this reason in the following we will concentrate
on the dilute limit below 1% and investigate it at low temperatures, where clustering eects
can be neglected.
120
80
40
0Ene
rgy
Shif
t (m
eV)
80604020Temperature (K)
0.5% Thallium(a) (b)
VB=170mV, It=1.95pA
Figure 6.2: Coverage calibration and temperature dependency. (a) Temperature dependenceof the doping eciency. The energy axis shows the energy shift of the Dirac point relativeto the clean graphene sample. (b) Topographic STM image of a Tl covered graphene surface(x = 0.2%) at a temperature of 4.5K. The Tl atoms appear as large protrusions with diameterof about 2 nm.
To support the assumption that we are dealing with isolated Tl atoms on the surface,
STM measurements were performed at very low temperatures in Vancouver. The mea
surements performed at 4.5K demonstrate that at very low concentrations Tl atoms are
present as immobile monomers on the surface [see Fig. 6.2(b)]. The topographic image
shows a Tl covered graphene monolayer. Even at a coverage of 0.2%, a small fraction of
adsorbed Tl appears to be in dimer or trimer form, however the vast majority appear to
be Tl monomers. Although the large size of the Tl adatoms and graphene's inherent elec
tronic inhomogeneity make an identication of the adsorption site dicult, Tl atoms on
more uniform graphene patches appear to sit on the hollow site, in agreement with density
54
6.2. Doping eect of Tl adatoms
functional theory (DFT) calculations [162]. As the precise coverage is important for the
subsequent quantitative analysis of the ARPES data, the STM results were also used for
the precise ux calibration of the Tl evaporator.
0.5
0.4
0.3
0.2
0.1
0.0
Energy Shift (eV
)
3210 Tl coverage x (%)
2
1
0
n (1
013cm
2)
calc. exp.0
.10.
00.
1M
omen
tum
(Å
1)
1.00.50Tl coverage x (%)
(a) (b)
Figure 6.3: Doping eect: (a) Evolution of the Fermi wave vector kF at K for increasing Tlcoverage x. (d) Charge carrier density, and experimental as well as calculated energy shift ofthe Dirac point as a function of Tl coverage x.
The shift of the Dirac point to higher binding energies upon Tl deposition illustrated
in Fig. 6.1 corresponds to an increase of the Fermi surface volume. The corresponding
evolution of Fermi wave vector kF , as well as the charge carrier density n and the energy
shift, are shown in Fig. 6.3(a) and (b), respectively. Below a coverage of 1%, all three
parameters increase monotonically. The energy shift reects the increase in occupation
due to the donation of electrons by the Tl atoms. A simple model employing graphene's
linear density of states serves to estimate the number of electrons donated per Tl atom η
via
x η =
∫ ExF
E0F
n(ε)dε, ∆E = ExF − E0
F
The Fermi level before and after the deposition is determined experimentally and the
coverage is known as well. The only free parameter is η. The best t for low coverages is
found for η = 1.0 electrons donated by a Tl atom to the graphene layer. This is also in
excellent agreement with recent DFT calculations for Tl adatoms on graphene [162].
55
Chapter 6. Scattering mechanisms in thallium doped epitaxial graphene
6.3 Linewidth analysis and theoretical description
In a Fermi liquid, linewidth broadening at the Fermi level due to interactions vanishes pro
portional to T 2 when the temperature goes to zero. Consequently, at a constant low tem
perature, linewidth broadening at the Fermi level from electronelectron, electronphonon
or electronplasmon interactions can be regarded as a small, constant contribution. Other
contributions are predominantly due to scattering from disorder such as impurities and
defects. To extract the scattering information we analyze the linewidth of the measured
spectra. The linewidths are taken from the FWHM of the MDCs at the Fermi level. We
tted the MDCs with a Voigt function and extracted the linewidths as a function of Tl
coverage as shown in Fig. 6.4(a). The width of the Gaussian resolution function was set to
match the experimental momentum resolution 0.016Å−1, while the linewidth, presented in
Fig. 6.4(b) corresponds to the FWHM of the Lorentzian lineshape.
Upon increasing Tl coverage, the linewidth increases monotonically. This is due to
scattering from the randomly adsorbed Tl atoms. We assume that the linewidth that we
measure for the clean sample comes from initial disorder, defects and residual interactions,
and enters as a constant oset in every measurement. This assumption is justied as long
as we stay at a constant low temperature, which results in small contributions from inter
actions. In order to unravel the contributions from the Tlinduced linewidth broadening
and thus the corresponding contribution to graphene's electrodynamics, we discuss two
scattering mechanisms in more detail.
6.3.1 Longrange scattering
Since Tl donates one electron per atom to the graphene sheet the atoms stay as charged
impurities on top. The rst mechanism that takes eect is scattering from charged impu
rities. Due to the screened Coulomb potential the Tl atoms show a longrange eect and
can be treated as longrange Coulomb scatterers. As described in Sec. 3.1.2, the linewidth
is proportional to the imaginary part of the selfenergy. Therefore, the linewidth broad
ening can be directly expressed via the imaginary part of the selfenergy for longrange
scattering [170]:
ImΣlong = α2nimpvFπI(2α)/kF (6.1)
where α is the eective nestructure constant, I(2α) is a function dened in [171], vF is
the Fermi velocity, nimp is the impurity density (which relates to the Tl concentration x
via nimp = 2x/A where A is the area of the graphene unit cell), and kF =√π(ηnimp + η0)
56
6.3. Linewidth analysis and theoretical description
is the Fermi momentum with η being the number of electrons donated per impurity atom,
and η0 the charge density in graphene before Tl deposition.
(a) (b)
0.60.40.20.0Tl coverage x (%)
0.035
0.030
0.025
0.020
0.015
Width (Å
1)
ε=7.26, δ=–3.2±1 eV ε=7.26, δ=0 eV ε=22, δ=0 eV experiment
Inte
nsity
(ar
b. u
nits
)
0.06 0 0.06k  kF (Å
1)
0.0%
0.1%
x=0.4%
Figure 6.4: Analysis of the experimental linewidth at the Fermi level. (a) Momentum distribution curves (MDCs) at the Fermi level for dierent Tl coverages x with the correspondingtted Voigt functions. (b) Increase of the linewidth as a function of Tl coverage x and theresults of the model calculations using dierent parameters. Due to the strongly nonlinearbehavior of the function the shaded green region is not symmetric around the green line.
The only free parameter in Eq. 6.1 is the eective nestructure constant of graphene;
all other parameters can be determined from the experiment. The eective ne structure
constant depends on the dielectric constant ε through α = 2.2/ε. The dielectric constant in
turn is determined by the underlying substrate; the smaller its value, the stronger the long
range scattering contribution to the linewidth broadening. From the analysis of plasmaron
signatures in epitaxial graphene on a buer layer on SiC(0001) [172], the dielectric constant
has been determined to be ε = 22 ± 8. Using this value of ε in Eq. 6.1, we calculated
the linewidth for longrange scattering. Starting with graphene's single particle Green's
function [173] we derived a theoretical spectral function by taking into account the self
energy [Eq. 6.1] and a constant oset for residual broadening. To be able to compare the
theoretical spectrum to the measured data we performed an analogous Lorentzian MDC
t procedure and determined the theoretical linewidth at the appropriate binding energy,
corresponding to the position of the Fermi level in the experiment. The resulting values
57
Chapter 6. Scattering mechanisms in thallium doped epitaxial graphene
are shown in Fig. 6.4(b) in red, and clearly do not t the measured linewidth evolution
with Tl coverage.
Recent calculations, however, point towards an overestimation of the dielectric constant
[174], suggesting that the actual value is likely smaller. Indeed, by analyzing the band
velocity renormalization in epitaxial graphene, a reduced value ε = 7.26± 0.02 was found
[175]. The linewidth broadening from longrange scattering for this value of the dielectric
constant is shown as a yellow line in Fig. 6.4(b). However, also this value of ε only accounts
for part of the experimental linewidth broadening. It is impossible to describe the data
in Fig. 6.4(b) without going to physically unreasonable values of ε. Therefore, another
mechanism is likely to contribute to the experimental linewidth.
6.3.2 Shortrange scattering
A second prominent scattering mechanism that arises in the presence of disorder is short
range scattering from an eective δpotential. Shortrange scattering is appreciable when
adatoms have states close to the Fermi level, thereby inducing a sizeable scattering potential
[167,176]. Its eect on the linewidth broadening can be modeled by the selfenergy within
the WolClogstonmodel [177, 178]. This approach does not distinguish between inter
and intravalley scattering in graphene, but it gives a general trend about the strength
of shortrange scattering. We adopt a selfconsistent implementation in the dilute limit
within the coherent potential approximation [179]
ImΣshort(ω) = x δ Im(
1 +δG0(ω − Σ(ω))
1− δG0(ω − Σ(ω))
)where G0(ω) is the lattice Green's function of the unperturbed graphene lattice [173] and
δ is the scattering potential. As Tl concentration x as well as the lattice Green's function
are known [the latter is displayed in Fig. 6.5(a)], the only free parameter in the shortrange
scattering model is the scattering potential parameter δ.
To evaluate the combined eect of both scattering processes, we add the selfenergies for
longrange and shortrange scattering, and calculate the theoretical linewidth like described
in Sec. 6.3.1. To this end, we note that ε and δ cannot be found simultaneously based on
our scattering analysis; however, using the experimentally determined value of ε from
Ref. [175], δ remains as the only unknown parameter and can thus be determined directly
from the observed linewidth evolution versus Tl concentration. We nd good agreement
with the experimental data for ε = 7.26 and δ = −3, 2 ± 1 eV [see shaded green area in
58
6.4. Graphene as topological insulator
Fig. 6.4(b)]. As it turns out, the contributions from shortrange and longrange scattering
have comparable magnitudes.
The overall behavior of the imaginary part of the shortrange scattering selfenergy for
graphene is shown in Fig. 6.5(b). Its rather strong energy dependence is due to the special
energy dependence of the graphene lattice Green's function in conjunction with that of the
scattering potential itself [Fig. 6.5(a)]. The dependence on the scattering potential δ at the
energy ω = 0.5 eV, thus in the vicinity of the experimentally relevant energies, is shown
in Fig. 6.5(c). For δ → ±∞, which can be interpreted as a missing atom in the lattice,
the imaginary part approaches the same nite value. For small values of δ, we see that
the imaginary part of the selfenergy varies more rapidly, although it remains bounded.
Therefore, the contribution from shortrange scattering to linewidth broadening is limited
for ω & 0.5 eV, but not necessarily negligible, and exhibits a maximum value for δ ≈ −5 eV.
When comparing the value obtained here for δ with available calculations in the lit
erature [162], we have to keep in mind that our shortrange scattering model does not
distinguish between dierent angular momentum channels, but rather attributes equal
scattering amplitude to all scattering channels. Nevertheless, we can estimate a value for
δ from the formula δ = t2ad/∆E, where tad is the hopping onto the Tl adatom and ∆E
is the energy dierence between the unperturbed and free Tl adatom states and the Fermi
level [167,176]. From the parameters reported in Ref. [162], we can estimate a theoretical
value δth ranging between −1 to −4 eV. Therefore, our results suggest that short range
scattering in this system lies on the larger side of the theoretically predicted range. Since
the resulting value for δ is close to the minimum of the imaginary part of the selfenergy
[see Fig. 6.5(c)], we expect a sizeable contribution of the shortrange scattering potential
to the linewidth broadening.
6.4 Graphene as topological insulator
Graphene was the rst material predicted to be a 2D TI, in which the SOC opens a band
gap at the Dirac point [31]. However, the SOC is very weak in carbon atoms and the
gap is unobservably small (∼ 10−3 meV). Further theoretical studies suggest that the gap
can be substantially enhanced by small amounts of adatoms on top of a graphene sheet.
As mentioned in Sec. 6.1, Tl was proposed to be the perfect candidate to increase the
SOC strength in graphene and induce a energy gap at the Dirac point [162]. By using
symmetry arguments, density functional theory (DFT), and tightbinding simulations the
59
Chapter 6. Scattering mechanisms in thallium doped epitaxial graphene
1.5
1.0
0.5
0.0
0.5
1.0
1.5
G0 (ω
) (e
V1
)
10 5 0 5 10EED (eV)
Re G0(ω)
Im G0(ω)
0.04
0.03
0.02
0.01
0.00
Im Σ
shor
t(ω
) (e
V)
10 5 0 5 10EED (eV)
x = 1%δ = 5eV
(a)
(b)
8
4
0
Im Σ
shor
t / x
(eV
)
20 10 0 10 20δ (eV)
ω=0.5 eV
(c)
Figure 6.5: Shortrange scattering model. (a) Real and imaginary part of the lattice Green'sfunction for graphene. (b) Imaginary part of the selfenergy for the short range scattering.(c) Selfenergy as a function of scattering potential δ at constant energy and normalized withrespect to the Tl coverage.
60
6.5. Discussion
authors predicted that Tl and In should be able to produce a substantial band gap on the
order of 21meV and 8meV, respectively, already at low coverages. However, there is no
experimental proof of that proposal so far. In contrast, our ARPES and some transport
measurements in Ref. [180] did not nd any indication for a gap at the Dirac point nor
a topological state. A robust topological phase in graphene would pave the way for a
new generation of spintronics devices and quantum information processing. However, our
ARPES and the transport measurements in Ref. [180] could not nd any indication for a
gap at the Dirac point nor a topological state.
6.5 Discussion
We have elucidated two dierent scattering mechanisms in Tl doped epitaxial graphene on
SiC(0001). Similar eects of enhanced scattering due to impurities have been observed in
a number of transport experiments [163, 181, 182], in agreement with our ndings. There,
the main scattering indicator is the carrier mobility, which decreases linearly with increas
ing impurity density. In contrast, a decreasing photoemission linewidth upon potassium
doping has been reported by Siegel et al. [157]. We attribute this variance to the dier
ent doping regime, and correspondingly dierent intrinsic screening, that were probed in
the experiments. Carrier scattering mechanisms in graphene (including charge impurities,
resonant scatterers, and ripples) have been strongly debated [163,183], and predominance
of one or the other mechanism is largely sample dependent. For graphene subjected to
charged impurities, e.g. alkali adatoms, longrange scattering is typically expected to be
much more eective in charge carrier scattering than short range scattering [181,184,185].
Tl adatoms on graphene, having an impurity charge of +1, might be expected to behave
in a similar fashion. We showed, however, that this is a system where both mechanisms
have nearly equal contributions due to the proximity of Tl states to the Fermi level. More
generally, this implies that it cannot be a priori assumed what scattering mechanism will
dominate in any given impuritygraphene system.
In summary, we used the experimental spectral function measured by ARPES on Tl
doped epitaxial graphene to observe the scattering behavior induced by the Tl adatoms,
and disentangle Coulomb (longrange) from δlike (shortrange) scattering contributions.
Exploiting the fact that correlation eects are suppressed at the Fermi level (Luttinger's
theorem), at low temperature the spectral linewidth at the Fermi level reects predom
inantly defect and disorder contributions. Both longrange and shortrange scattering
61
Chapter 6. Scattering mechanisms in thallium doped epitaxial graphene
mechanisms can be described by an analytic expression for the selfenergy in the dilute
limit. Fitting the selfenergy to the experimental data allowed us to extract the fundamen
tal parameters of the scattering mechanisms at play in the graphene layers.
62
Chapter 7
Circular dichroism in the band
structure of surface alloys
Changing the photon source from nonpolarized light to linearly or circularly polarized
light in an ARPES experiment aects the measured photocurrent considerably. For dier
ent polarizations dipole selection rules lead to dierent cross sections for the interaction
between polarized light and matter. Recently, ARPES setups combined with a circularly
polarized light source are seen to be a perfect tool to measure the chiral spin structure of
surface states [186189]. Our CD measurements on surface alloys on Ag(111), however,
show that CD is strongly dependent on the photonenergy and contains only indirect infor
mation about the spin structure. Instead of following the spin direction, CD is dominated
(i) by the geometry of the experimental setup, (ii) by the dipole selection rules and hence
by the OAM and (iii) by the nal state. In TIs for example the spin is aligned with the
OAM due to the very strong SOC [190192]. As long as nal state eects do not enter, the
CD signal shows twofold symmetric structures that can be mistaken for the z component
of the spin.
In the following section, we will introduce the concept of CD. After the presentation of
our results from the measurements on the surface alloys we will discuss possible interpre
tations. At the end, we address the question of whether there is a chance to obtain access
to the spin polarization of surface states via CD measurements.
63
Chapter 7. Circular dichroism in the band structure of surface alloys
7.1 Circular dichroism in the angular distribution of
photoelectrons
In general, CD is the dierence in the absorption of lefthanded circularly polarized light
(LCP) and righthanded circularly polarized light (RCP). It is known from chiral molecules
that they show selective absorption of RCP and LCP. Dichroic signals are also used in X
ray magnetic circular dichorism (XMCD) experiments, where the dierence spectrum of
two xray absorption spectra is taken in a magnetic eld. This technique gives access to
the magnetic properties of an atom or a molecule. Information about spin and orbital
magnetic moment can be obtained. But even if magnetic eld and chiral sample are
absent, dichroism eects can still be observed. For ARPES measurements the dierence of
the photoemission spectra for both polarizations is taken and the measured signal is called
'circular dichroism in the angular distribution of the photoelectrons'. The most important
requirement for a dichroic signal is a denite handedness of the combined system of photons
and reaction partner. If the sample itself is nonchiral, the experimental geometry can still
induce chirality. In principle every crystal shows CD eects if the direction of photon
impact ~q, photoelectron momentum ~k and surface normal ~n are noncoplanar [193].
To gain information about the spin of a system with ARPES, the interaction between
light and matter in the experiment has to be spindependent. Using circularly polarized
light and changing the polarization provides the possibility to induce a spin dependency.
There are two proposals for spindependent interaction Hamiltonians, where the authors
claim to measure the spin signal of the surface states ( [186] and [187]). However, in both
models assumptions about the geometry of the sample or about the spin polarization of
the bands are necessary.
For the interpretation of CD data, it is important to understand its origin. Presumably
SOC plays an important role. However, it is denitively not the only ingredient because
also very light atoms show a strong CD eect e.g. graphene [194]. There are also other
factors that have an inuence on the CD signal, like the geometrical setup [193] and the
photon energy [195], which were so far mainly ignored by the community. Recently, it was
proposed that the CD signal is proportional to the OAM [196]. Based on this fact the
question arises whether it is actually possible to probe the spin of the initial state with
CDARPES.
64
7.2. Photoemission experiments
7.2 Photoemission experiments
We performed ARPES experiments with circularly polarized light on Bi/Ag(111) and
Sb/Ag(111) surface alloys. The measurements were performed at the Synchrotron Ra
diation Center (SRC) in Stoughton, Wisconsin [for details see Sec. 3.2]. A sketch of the
experimental setup is displayed in Fig. 7.1.
sample
θin
ciden
t lig
ht RCP
LCP
photoelectrons
50°
analyzer
Figure 7.1: Sketch of the experimental setup for CD measurements.
For RCP (LCP) light the electric eld vector rotates anticlockwise (clockwise) around
the direction of light propagation. In order to measure the photoemission current as a
function of ky the sample was rotated by an angle θ [see Fig. 7.1]. kx (direction perpendic
ular to the paper plane in Fig. 7.1) corresponds to the angular dispersion direction in the
2D detector.
To prepare the surface alloys the Ag(111) substrate has to be cleaned by several sputter
ing/annealing cycles. We sputtered the surface with Ar ions with an energy of 1 keV and at
an Ar pressure of 1·10−6 mbar and subsequently annealed the sample at 530C. Cleanliness
of the substrate was controlled by monitoring the surface state of Ag(111) with ARPES.
On the clean Ag(111) surface one third of a monolayer of Bi or Sb is deposited using a
commercial electron beam evaporator. The Ag crystal was kept at 420C and 250C for Bi
and Sb deposition, respectively. For the measurements, the sample temperature was∼50K.
In Fig. 7.2 the results of the ARPES measurements are shown for RCP and LCP light
as well as the dierence (CD) in ΓM direction of the Bi/Ag(111) surface alloy measured
with a photon energy of hν = 29 eV.
The 2D band structure in surface alloys on Ag(111) consists of three sets of spinsplit
65
Chapter 7. Circular dichroism in the band structure of surface alloys
0.2 0.1 0.0 0.1 0.2kx (Å
1)
0.2 0.1 0.0 0.1 0.2kx (Å
1)
1.0
0.8
0.6
0.4
0.2
0.0
0.2
Initi
al s
tate
ene
rgy
(eV
)
0.2 0.1 0.0 0.1 0.2kx (Å
1)
RCP LCP CDΓM
Figure 7.2: Band structure of Bi/Ag(111): The spectra are measured in ΓM direction at aphoton energy of hν = 29 eV for RCP and LCP, on the left and in the middle, respectively.The right panel show the intensity dierence (CD= IRCP − ILCP ). Red (blue) correspondsto positive (negative) values, white corresponds to zero.
bands; one at lower binding energy with mainly spz character, two at higher binding energy
with mainly pxy character and mj = 1/2; 3/2 [66]. The measurements of Bi/Ag(111) show
the known, large spin splitting of the lowest band [63]. The intensity of the parabolas
varies strongly with the polarity of the light. Parts of the band structure are only visible
for RCP and others only for LCP light. By taking the dierence one gets the CD image,
in which each parabola of the spz spinpolarized band has its own color. Red (blue) means
the intensity for RCP (LCP) light was higher and white means that the intensity was the
same for both polarizations. Close to the Fermi energy we see that also the pxy bands show
a CD signal.
Fig. 7.3 shows ARPES results for the same measurements conditions but for Sb/Ag(111).
The atomic SOC in Sb is much weaker. Therefore, the spin splitting is much smaller and
we do not resolve it in the spz band, but we see just one parabola. Nevertheless, we observe
a clear dichotomy in the CD signal. Despite the fact that the band is spin degenerate it is
bicolored in the CD image and gives us direct proof that CD cannot be an independent,
direct measure for the spin structure.
Measured constant energy planes for both alloys at EB = 0.6 eV are displayed in Fig.
7.4. The measurements show that CD vanishes in ΓK direction. For Bi/Ag(111) only the
inner band is visible at this energy and shows a twofold symmetry. In the case of Sb both
66
7.3. Theoretical description
0.2 0.1 0.0 0.1 0.2kx (Å
1)
0.2 0.1 0.0 0.1 0.2kx (Å
1)
1.0
0.8
0.6
0.4
0.2
0.0
0.2
Initi
al s
tate
ene
rgy
(eV
)
0.2 0.1 0.0 0.1 0.2kx (Å
1)
LCP CDΓMRCP
Figure 7.3: Band structure of Sb/Ag(111): The spectra are measured in ΓM direction at aphoton energy of hν = 29 eV for RCP and LCP, on the left and in the middle, respectively.The right panel show the intensity dierence (CD= IRCP − ILCP ). Red (blue) correspondsto positive (negative) values and white to zero.
bands are visible. For the inner band the dichotomy is clearly conrmed, but the CD signal
of the outer band changes sign four times on a circle around Γ. The dierence between
both bands is the orbital character. We observe that dierent initial states give rise to CD
signals with dierent symmetries.
7.3 Theoretical description
In order to explore the origin of CD and explain our observations, we take a very sim
ple approach, i.e. the model for CD of Schönhense [193]. This model states, that in
principle, every crystal shows CD if the criterion for the appearance of CD eects is ful
lled; the direction of photon impact ~q, photoelectron momentum ~k and surface normal
~n must be noncoplanar. For the calculation of the transition matrix element the elec
tric dipole operator for RCP and LCP and the corresponding selection rules are taken.
The nal state is expressed as a partial wave expansion and can be written as Ψf =
4π∑l′m′
FEl′(r)(i)l′e−iδl′Y ∗l′m′(k)Yl′m′(r). Here, l′ gives the orbital of the nal state, FEl′
stands for the radial wave functions, δl′ represents the phase shifts experienced by the
outgoing partial waves, and k and r specify the photoelectron emission direction and the
67
Chapter 7. Circular dichroism in the band structure of surface alloys
0.3
0.2
0.1
0.0
0.1
0.2
k y (
Å1
)
0.2 0.0 0.2
kx (Å1
)
0.1
0.0
0.1k y
(Å
1)
0.2 0.0 0.2
kx (Å1
)
Figure 7.4: Measured constant energy planes cut through the band structure of Bi/Ag(111)(left) and Sb/Ag(111) (right) at EB = 0.6 eV as indicated in the CD images in Fig. 7.2 andFig. 7.3.
direction of the position vector, respectively. Sorbitals do not give any contribution to
the CD signal because of their spherical symmetry that cancels out all CD eects. If we
consider the geometry of our experimental setup, including the direction of light incidence
(50− θ) and of electron detection (θ;φ), we nd the following CD signal depending on the
initial state [193,197]:
CD(px) ∝−RsRd
2πsin(δs − δd) sin2(θ) sin(2φ) cos(50 − θ)
CD(py) ∝+RsRd
πsin(δs − δd) sin(θ) sin(φ)×
(sin(θ) cos(φ) cos(50 − θ) + cos(θ)sin(50 − θ))
CD(pz) ∝−RsRd
2πsin(δs − δd) sin(2θ) sin(φ) sin(50 − θ)
with the radial part of the matrix elements Rs and Rd. These equations are plotted in Fig.
7.5.
Like in our experimental data, the simple model calculations show also that in ΓK
direction there is no CD signal. The reason for no signal at kx = 0 is the symmetry of the
orbitals and the experiment. Symmetry also requires that the sum over all porbitals gives
zero. The calculations conrm that dierent initial states lead to dierent symmetries in
the CD signals: CD of the pz and py orbital is at rst sight twofold symmetric whereas
68
7.4. Orbital angular momentum in surface alloys
0.2 0.0 0.2
kx (Å1
)
0.2 0.0 0.2
kx (Å1
)
0.2
0.1
0.0
0.1
0.2
k y (
Å1
)
0.2 0.0 0.2kx (Å
1)
px py pz
Figure 7.5: Results of the model calculations using Schönhenses model combined with thegeometry of the experimental setup for a px, py or pz orbital as initial state from left to right,respectively.
the px shows a fourfold symmetry. This agrees very much with our measurements where
the spz band changes sign two times and the pxy band four times on a circle around Γ.
Overall, the simple theoretical ndings are in very good agreement with our experimental
observations.
7.4 Orbital angular momentum in surface alloys
So far, our observations t also very well to those of Kim et al. [198] and of Park et al. [191].
They performed DFT and rstprinciples calculations and showed that CD follows the
OAM. The OAM, in combination with the electron momentum ~k, leads to small electric
dipoles (asymmetric charge distribution) that have opposite orientation for opposite OAM
directions. The surface electric eld aligns the electric dipoles and splits the states through
the electric dipole interaction.
The alignment of the spin angular momentum (SAM) is a consequence of strong SOC
and the chiral OAM structure: For small SOC the spin moment is either parallel or anti
parallel to the OAM. For strong atomic SOC, however, the OAM is always pointing in the
opposite direction of the SAM and the bands show a signicant spin splitting. Exactly this
has been observed in our measurements; in Sb/Ag(111) the OAM is parallel for both bands
(spin splitting is not resolved in our experiments) because the SOC is too weak to align
the SAM and OAM. The situation in Bi is dierent; there, SOC is strong enough to align
SAM and OAM. The spin is pointing antiparallel for the inner and the outer band and the
69
Chapter 7. Circular dichroism in the band structure of surface alloys
OAM follows this structure with the opposite sign. For the inner band we observe a CD
signal where the intensity varies proportional to a sinusoidal curve on a circle around Γ.
This is shown for the case of Bi/Ag(111) and hν = 25 eV in Fig. 7.6. Due to the similarity,
such a signal is often misinterpreted as proof of the chiral structure in the SAM [27].
0.3
0.2
0.1
0.0
0.1
0.2
k y (
Å1
)
0.20.10.00.10.2
kx (Å1
)
φ
0.3
0.2
0.1
0.0
0.1
0.2
0.3
NC
D
0 π/2 π 3/2 π 2πφ
(a) (b)
Figure 7.6: Normalized CD signal on a circle around Γ (a) Measured constant energy planecut through the band structure of Bi/Ag(111) at EB = 0.6 eV with hν = 25 eV (b) Absolutevalues of the normalized CD signal on a circle indicated in (a) around Γ.
7.5 Photonenergy dependence
We have seen that SOC plays a crucial role for CD measurements and that the CD signal
follows mainly the OAM. Additionally, the experimental setup is just as important as
the last ingredient; the photon energy. The choice of the photon energy determines the
nal state in which the excited electron goes. According to the dipole selection rules
combined with circularly polarized light only certain transitions are allowed. Depending
on the energy, dierent nal states are available and the corresponding CD signal can
change completely. It can vanish or even reverse its sign. Fig. 7.7 shows the CD signal for
dierent photon energies (25 eV, 45 eV and 90 eV) of Bi/Ag(111).
The data show the normalized CD signal NCD = (IRCP−ILCP )/(IRCP +ILCP ), which is
the dierence of the measured spectra divided by the sum. The sign of NCD in the spz band
changes for dierent photon energies. At hν = 25 eV and a binding energy of EB = 0.6 eV
the left branch is red, i.e. the intensity for RCP light was higher. For 45 eV and 90 eV it
70
7.5. Photonenergy dependence
1.0
0.8
0.6
0.4
0.2
0.0
0.2
Initi
al S
tate
Ene
rgy
(eV
)
0.2 0.1 0.0 0.1 0.2
kx (Å1
)
0.2 0.1 0.0 0.1 0.2
kx (Å1
)
hν=25eVBi/Ag(111) 45eV
0.2 0.1 0.0 0.1 0.2
kx (Å1
)
90eV
Figure 7.7: CD signal of the band structure in Bi/Ag(111) for dierent photon energies.Changing the energy results in a change of the nal state symmetry and thus in a change ofthe sign of the CD signal. Matrix elements eects lead to dierent intensity patterns. Thecolor code goes from blue (0.6) to red (0.6).
is blue and the intensity for LCP was higher. In order to evaluate this quantitatively we
extracted the maximum value of the normalized CD at an MDC at EB = 0.6 eV for both
branches. The result is presented in Fig. 7.8.
From this plot it can be easily seen that nal state eects play the most important
role in CD measurements and in the data interpretation [195]. In the energy window from
25 eV to 90 eV, the CD changes sign several times. For some energies CD even vanishes
(see the spz band at 45 eV above the crossing point). Despite this strong inuence, nal
state eects and the resulting photon energy dependence have rarely been discussed by the
community to date. The usual approach was always to explain CD by various initialstate
models favoring the spin or OAM as origin for CD. However, none of these can describe
all the experimental observations and nal state eects have to be considered [195].
Even in the simple model of Schönhense, the sign change due to the nal state is
included via the factor sin(δs − δd). In our experiments we found even a case where the
CD signal changes sign within one branch for the same photon energy. For example, for
Sb/Ag(111) at hν = 55 eV [see Fig. 7.9]. Such a sign change was also observed in Ref. [190]
and calculated in Ref. [192]. Also this phenomenon can only be explained by a transition
into a new nal state.
71
Chapter 7. Circular dichroism in the band structure of surface alloys
0.6
0.4
0.2
0.0
0.2
0.4
0.6
norm
aliz
ed C
D
90807060504030Photon Energy (eV)
Figure 7.8: Photon energy dependence of the band structure in Bi/Ag(111). The maximumvalue of the normalized CD in both branches of the spz band at EB = 0.6 eV is shown. Thenormalized CD changes sign at several photon energies.
7.6 Discussion
The presented ARPES study with circularly polarized light shows that the photon energy
plays a very important role for the interpretation of CD data. To describe the experimental
data the model of Schönhense [193] is very useful. In this model CD is a consequence of the
interaction of circularly polarized light and the electrons in the surface. The measured CD
signal is a combination of the OAM superposed with geometrical and nal state eects. If
we know the nal state and consider carefully the geometrical setup of the experiment, we
are able to measure the OAM with an ARPES setup combined with a circularly polarized
photon source. In case of strong SOC we can even obtain information about the SAM,
because high SOC leads to aligned SAM and OAM. However, there are also examples for
spin resolved ARPES measurements where nal state eects perturb the experiment [199].
In order to improve the quantitative explanation of the measured CD signal several
possibilities are discussed in literature. It was claimed [186] that the experimental geometry
induced matrix element eects can be eliminated by using a timeofight detector and
measuring the whole band structure simultaneously without turning the sample. This is
only true under certain circumstances because even in this setup the CD signal is aected
by geometry since the direction of photon impact ~q, photoelectron momentum ~k and sample
normal ~n are still noncoplanar for most values of ~k. The only way remove of the geometric
contribution to the CD signal is to apply symmetry properties and taking the dierence
between CD signals measured ∆φ = 60C apart [186]. This procedure might even allow for
72
7.6. Discussion
1.0
0.8
0.6
0.4
0.2
0.0
0.2
Initi
al s
tate
ene
rgy
(eV
)
0.2 0.0 0.2
kx (Å1
)
hν=55eV
Figure 7.9: Band structure of Sb/Ag(111) at hν = 55 eV at Γ. CD signal changes its signwithin the band.
a determination of the 3D spin polarization vector. But this eect has not been investigated
as a function of photon energy so far. The simple Schoönhense model has both eects
included: geometry and nal states. But the biggest problem is the initial state. Since the
dierent bands are not purely s or p bands but have dierent orbital character it is dicult
to nd a description for a realistic initial state. We claim that the model would probably
give a more sophisticated result for the CD signal if a more realistic initial and nal state
wave function is inserted.
In conclusion, we can state that analysis and interpretation of CD data has to be at
tempted with caution. They do not give direct access to the spin structure of surface states.
What CDARPES experiments rather measure seems to be the OAM, but superposed with
geometrical and nal state eects. In the presence of high SOC the spin aligns with the
OAM (either parallel or antiparallel) and one might say that CD burrows the electron
spin but it does not give direct access to it.
73
Chapter 7. Circular dichroism in the band structure of surface alloys
74
Chapter 8
Summary and Outlook
8.1 Summary
In this work, we have investigated several 2DESs and studied in particular the electronic
properties at the surface of TiTe1.5Se0.5 and signatures of manybody physics in Bi2Te2Se
and graphene. We showed that interactions play an important role, not only for the Dirac
electrons in graphene but also for the spinpolarized surface states of 3D TIs. In addition,
we also evaluated CDARPES as a technique to measure spinsplit surface states and in
order to get information about the initial state properties.
In the rst part we focused on topological nontrivial surface states and their character
istics. We measured the surface band structure of Bi2Te2Se and observed a timedependent
doping behavior due to adsorption of residual gas molecules. By a careful analysis of the
position and the linewidth of the peaks in the measured spectra we found that the band
structure is strongly renormalized while the charge carrier density n is changing. The
linewidth is increasing with increasing binding energy and the band velocity is smaller for
low n. These observations can be explained by the strong Coulomb interaction among the
electrons, since at very small n screening eects are not ecient.
We did not just investigate known TIs but have also looked for new topological materi
als. Therefore, we had a look at a system that is expected to exhibit a topological surface
state. We measured the surface band structure on mechanically cleaved single crystals of
TiTe1.5Se0.5 and could present the band dispersion for the rst time. The bands disperse
as expected and the inverted band gap lies above the Fermi. Since ARPES is only sensitive
to the occupied states we were not able to measure any topological surface state, but the
material looks like a promising TI candidate.
75
Chapter 8. Summary and Outlook
In the second part we studied scattering mechanisms in a doped monolayer of epitaxial
graphene grown on a buer layer on SiC(0001) by depositing Tl adatoms. To overcome the
high mobility of Tl adatoms, we deposited them and performed the measurements at very
low temperatures. We have quantitatively shown that Tl adatoms not only show electron
doping up to a certain coverage, but also have a large eect on the quasiparticle scattering
rate. The Tl adatoms introduce disorder and act on the graphene electronic structure both
as Coulomb longrange scatterers as well as shortrange scatterers with a δlike potential.
By modeling the selfenergy for both scattering mechanisms, we are able to extract a
strong shortrange scattering potential δ = −3.2 ± 1 eV. Thus, shortrange scattering can
contribute to a sizeable increase of the scattering rate, even in the case of charged impurities
where longrange Coulomb scattering is usually expected to dominate. These ndings,
and the ability to predict and/or account for conating scattering mechanisms, will have
important implications in the development of novel impuritygraphenebased electronics.
At last we had a closer look at ARPES measurements with circularly polarized light.
By investigating two systems with dierent SOC strengths Bi/Ag(111) and Sb/Ag(111)
surface alloys we were able to gain a deeper insight into the details and the challenges
of CDARPES. We observed that CD follows not the SAM but more the OAM. A quite
simple model based on the geometry and the selection rules describes the basic eects very
well [27, 193]. However, we also found that the photon energy has a big impact on the
measurements. For a proper interpretation of CD signals one has to consider not only
the OAM of the initial state, but also the geometry of the experimental setup as well as
the photon energy and thus nal state eects. It is impossible to draw reliable general
conclusions about the spin texture from CD measurements.
8.2 Outlook
In this section, some possible followup experiments and ideas for proceeding are given.
Further, we will present some potential applications of the investigated materials.
Much of the theoretical research on Dirac electrons has focused on the singleparticle
picture since the basic physical phenomena can be calculated and explained very well
both in the spindegenerate case graphene as well as in the spinpolarized surface
states of TIs. For example, the band structure [39], the integer quantum Hall eect [200],
localization [201], and topological classication [202] are very well described in theory
without interactions. However in the case of graphene, ARPES experiments [101,157,172,
76
8.2. Outlook
203] have directly shown the existence of manybody quasiparticle spectra near the Dirac
point, manifesting electronelectron, electronphonon, and electronplasmon interactions.
It was proven that interactions under certain circumstances play an important role and
can change the physical picture drastically.
8.2.1 Topological insulators
Recently, some experimental work on manybody interactions in TIs has also been per
formed. For example, Park et al. [204] investigated the electronelectron interaction and
defect scattering in Bi2Se3 and claimed that topological states could be indeed protected
against weak perturbations. They showed that topological metallic states are very much
unaected by the potentials created by adsorbed atoms or molecules. Transport measure
ments on TI thin lms could demonstrate that the interplay between topological delo
calization, electron interaction, and broken timereversal symmetry play a crucial role in
determining the transport properties of the TI thin lms [205]. The authors addressed the
question whether topological surface states are topologically protected from localization
and remain metallic down to zero temperature. Up to a thickness of 6 quintuple layers,
they observed an insulating ground state due to electronelectron interactions, which is
enhanced by the diusive nature of electron motion in disordered thin lms.
It was also shown that electronelectron interactions lead to localization of the elec
trons [206] and can even destroy the topological character [6]. In particular, for very
low charge carrier densities and low dielectric constants, electronelectron interactions in
TIs are not negligible [59], as was also shown in this work. Interactions lead to a more
complex physical picture and make the description often dicult, but usually they also
introduce new possibilities. For example, superconductivity was predicted in Bi2Se3 due
to electronphonon interactions with a critical temperature of TC = 1K. Including quasi
particle dynamics in Dirac electrons of TIs will be one important subject for upcoming
experiments and theoretical studies in the eld of TIs. The motivation is still to under
stand what turns a material into a TI and to nd new topological materials with intriguing
properties that are suitable for potential applications. In particular, the electronic prop
erties of TIs hold a great potential for spintronics applications and quantum information
processing [207].
For our studies, rst of all it would be desirable to conrm our ndings by a theoretical
description that relates the electronelectron interaction constant β and the determined
ratio β1/β2 to the dielectric constant ε and the charge carrier density n. Therefore, it
77
Chapter 8. Summary and Outlook
is necessary to repeat the measurements at low temperature, which allows one to also
estimate the contribution from electronphonon interaction. Furthermore, the transfer of
this method to other topological materials that have only surface states at the Fermi level
is planned. For the promising TI candidate TiTe1.5Se0.5, the next step would be to dope
the system with some electrons in order to shift the inverted band gap into the occupied
states. For example, Na could be a possible electron donor since it donates quite easily
electrons without disturbing the electronic properties [166]. Furthermore, it was shown
that Na can lead to energy shifts of about 0.5 eV. In addition, another possible experiment
would be to measure also CDARPES on both topological materials.
8.2.2 Circular dichorism measurements
The determination of the spin texture of TIs is still of paramount importance for both
fundamental understanding of its topological order and future spinbased applications. In
this context, much experimental work on TIs was performed with spinresolved ARPES and
CDARPES. There are numerous proposals to use circularly polarized light to selectively
couple to the surface states to generate surface spin waves [208] or spinpolarized currents
[209]. By tuning the light polarization it was claimed that TIs may serve as spinpolarized
electron sources [210]. As a consequence of the large OAM very strong spinpolarized
currents in surface states can be induced by light. Following the dipole selection rule, an
electron with sorbital character can be excited by a photon to the porbitals in the surface
states. Using circularly polarized photons allows one to excite electrons only in a certain
part of the Brillouin zone with the proper OAM. Since the surface states are spinpolarized,
selective excitation of electrons should result in spinpolarized current [191].
In particular, for the surface alloys on Ag(111) it would be desirable to observe the
transition of parallel to antiparallel OAM in the surface states. It was shown that mixing
of the alloy atoms allows tuning of the Fermi level and of the SOC strength [211]. With
the proper ratio of Bi and Sb atoms one should be able to reach the point where the OAM
is reversed for one of the bands. This would serve as perfect proof that CDARPES probes
in principle the OAM.
8.2.3 Graphene
The knowledge we gained in our experiments with graphene is very exciting from a funda
mental point of view. With our technique we are able to determine the scattering potential
78
8.2. Outlook
of shortrange scattering centers. It would be interesting to investigate also other adatoms
or adsorbates with regard to their scattering potential. One could also think of modifying
the dielectric properties of graphene by intercalating elements and check the dierence in
the linewidth broadening for dierent dielectric constants ε.
The ultimate goal in the research eld of graphene is still to use it in electronic devices
one day. Since graphene is a semimetal, where the conduction and the valence band are
touching at the Kpoints, it lacks a band gap which leads to comparatively low ono
ratios in graphene based eld eect transistors. A lot of eort has been directed towards
the opening of an energy gap at the Dirac point [75,102,212215]. For example, such a band
gap was realized in graphene nanoribbons due to quantum connement of the electrons.
Also, our experiments and some transport measurements [180] have aimed in this direction.
Unfortunately, the theoretical predictions could not be proven, so far. However, there are
already some new ideas about the gapopening in graphene via SOC. In Ref. [216] the
authors claim that a small amount of 5d transition metal atoms, in particular Osmium
and Iridium, on top of graphene will open an even bigger gap at the Dirac point. They
suggest to build a 2D TI by hybridizing graphene with impurity bands arising from heavy
adatoms possessing partially lled d shells. By means of rstprinciples calculations they
predict gaps of 0.2 eV and larger over a wide range of adatom coverage.
Figure 8.1: Schematic representation of δgraphyne taken from [217]. The unit cell with thetwo basis vectors ~a1 and ~a2 are indicated by the red lines. According to the dierent chemicalenvironments the carbon atoms are drawn in dierent colors.
Recently published theoretical work has proposed a new 2D TI made out of carbon [217].
The socalled graphynes, which are carbon allotropes built from triple and doublebonded
units of carbon atoms, were considerably investigated and show interesting properties. In
particular, δgraphyne [drawn in Fig. 8.1] was predicted to show a topologically nontrivial
electronic structures. The energy band gap of δgraphyne is still quite small (0.59meV)
79
Chapter 8. Summary and Outlook
but could be experimentally accessible at extremely low temperatures. This approach
demonstrates promising possibilities for the search for new TIs in 2D carbon allotropes.
Realization of these proposals would open the door for realizing topological super
conductivity, Majorana fermions, and related phenomena. It is worth mentioning, that
one of the primary requirements for observing those eects is to induce superconduc
tivity in graphene via the proximity eect, which has already been shown by several
groups [218220].
80
Bibliography
[1] M. Schroeder Fractals, chaos and power laws, W. H. Freeman and Company (1991)
[2] K. v. Klitzing, G. Dorda, and M. Pepper `New method for highaccuracy determi
nation of the nestructure constant based on quantized hall resistance' Phys. Rev.
Lett. 45, 494 (1980)
[3] J. Sinova, D. Culcer, Q. Niu, N. A. Sinitsyn, T. Jungwirth, and A. H. MacDonald
`Universal intrinsic spin Hall eect' Phys. Rev. Lett. 92, 126603 (2004)
[4] J. Wunderlich, B. Kaestner, J. Sinova, and T. Jungwirth `Experimental observation
of the spinHall eect in a twodimensional spinorbit coupled semiconductor system'
Phys. Rev. Lett. 94, 047204 (2005)
[5] Y. Ando `Topological insulator materials', J. Phys. Soc. Jpn. 82, 102001 (2013)
[6] M. Liu, C.Z. Chang, Z. Zhang, Y. Zhang, W. Ruan, K. He, L.l. Wang, X. Chen,
J.F. Jia, S.C. Zhang, Q.K. Xue, X. Ma, and Y. Wang `Electron interactiondriven
insulating ground state in Bi2Se3 topological insulators in the twodimensional limit',
Phys. Rev. B 83, 165440 (2011)
[7] Y. A. Bychkov and E. I. Rashba `Properties of a 2D electron gas with lifted spectral
degeneracy', JETP Lett. 39, 78 (1984)
[8] C. Kittel, Einführung in die Festkörperphysik, Oldenbourg Verlag (2002)
[9] I. Gierz, Investigation of twodimensional electron gases with angular resolved photoe
mission spectroscopy Ph.D. thesis, Ecole Polytechnique Fédérale de Lausanne (2011).
[10] K. S. Novoselov, Z. Jiang, Y. Zhang, S. V. Morozov, H. L. Stormer, U. Zeitler, J. C.
Maan, G. S. Boebinger, P. Kim, and A. K. Geim `Roomtemperature quantum hall
eect in graphene', Science 315, 1379 (2007)
81
Bibliography
[11] K. Oura, V. G. Lifshits, A. A. Saranin, A. V. Zotov, and M. Katayama Surface
Science An Introduction, Springer Berlin (2003)
[12] W. Shockley `On the surface states associated with a periodic potential', Phys. Rev.
56, 317 (1939)
[13] I. Tamm `Über eine mögliche Art der Elektronenbindung an Kristalloberächen',
Zeitschrift für Physik 76, 849 (1932)
[14] H. Kramers `General theory of the paramagnetic rotation in crystals', Proceedings
of the Section of sciences Koninklijke Nederlandse akademie van wetenschappen 33,
959 (1930)
[15] J. Nitta, T. Akazaki, H. Takayanagi, and T. Enoki `Gate control of spinorbit inter
action in an inverted In0.53Ga0.47As/In0.52Al0.48As heterostructure', Phys. Rev. Lett.
78, 1335 (1997)
[16] E. Frantzeskakis and M. Grioni `Anisotropy eects on Rashba and topological insu
lator spinpolarized surface states: A unied phenomenological description', Phys.
Rev. B 84, 155453 (2011)
[17] U. Heinzmann and J. H. Dil `Spinorbitinduced photoelectron spin polarization
in angleresolved photoemission from both atomic and condensed matter targets',
Journal of Physics: Condensed Matter 24, 173001 (2012)
[18] G. Dresselhaus `Spinorbit coupling eects in zinc blende structures', Phys. Rev.
100, 580 (1955)
[19] E. I. Rashba `Properties of semiconductors with an extremum loop .1. cyclotron and
combinational resonance in a magnetic eld perpendicular to the plane of the loop',
Sov. Phys. Solid State 2, 1109 (1960)
[20] D. Di Sante, P. Barone, R. Bertacco, and S. Picozzi `Electric control of the giant
Rashba eect in bulk GeTe', Advanced Materials 25, 509 (2013)
[21] Y. A. Bychkov and E. I. Rashba `Oscillatory eects and the magnetic susceptibility
of carriers in inversion layers', J. Phys. C: Solid State Phys. 17, 6039 (1984)
82
Bibliography
[22] S. LaShell, B. A. McDougall, and E. Jensen `Spin splitting of an Au(111) surface
state band observed with angle resolved photoelectron spectroscopy', Phys. Rev.
Lett. 77, 3419 (1996)
[23] D. Popovic, F. Reinert, S. Hüfner, V. G. Grigoryan, M. Springborg, H. Cercellier,
Y. FagotRevurat, B. Kierren, and D. Malterre `Highresolution photoemission on
Ag/Au(111): Spinorbit splitting and electronic localization of the surface state',
Phys. Rev. B 72, 045419 (2005)
[24] F. Forster, S. Hüfner, and F. Reinert `Rare gases on noblemetal surfaces: An angle
resolved photoemission study with high energy resolution', J. Phys. Chem. B 108,
14692 (2004)
[25] L. Petersen and P. Hedegård `A simple tightbinding model of spinorbit splitting of
spderived surface states', Surface Science 459, 49 (2000)
[26] R. Winkler Spinorbit coupling eects in twodimensional electron and hole systems,
Springer Berlin (2003)
[27] S. R. Park, C. H. Kim, J. Yu, J. H. Han, and C. Kim `Orbitalangularmomentum
based origin of Rashbatype surface band splitting', Phys. Rev. Lett. 107, 156803
(2011)
[28] I. Gierz, B. Stadtmüller, J. Vuorinen, M. Lindroos, F. Meier, J. H. Dil, K. Kern, and
C. R. Ast `Structural inuence on the Rashbatype spin splitting in surface alloys',
Phys. Rev. B 81, 245430 (2010)
[29] I. Gierz, T. Suzuki, E. Frantzeskakis, S. Pons, S. Ostanin, A. Ernst, J. Henk, M. Gri
oni, K. Kern, and C. R. Ast `Silicon surface with giant spin splitting', Phys. Rev.
Lett. 103, 046803 (2009)
[30] S. Datta and B. Das `Electronic analog of the electrooptic modulator', Applied
Physics Letters 56, 665 (1990)
[31] C. L. Kane and E. J. Mele `Quantum spin hall eect in graphene', Phys. Rev. Lett.
95, 226801 (2005)
[32] B. A. Bernevig, T. L. Hughes, and S.C. Zhang `Quantum spin hall eect and
topological phase transition in HgTe quantum wells', Science 314, 1757 (2006)
83
Bibliography
[33] M. König, S. Wiedmann, C. Brüne, A. Roth, H. Buhmann, L. W. Molenkamp, X.L.
Qi, and S.C. Zhang `Quantum spin hall insulator state in HgTe quantum wells',
Science 318, 766 (2007)
[34] S. Chadov, X. Qi, J. Kübler, G. H. Fecher, C. Felser, and S. C. Zhang `Tunable
multifunctional topological insulators in ternary Heusler compounds', Nat. Mater.
9, 541 (2010)
[35] L. Fu, C. L. Kane, and E. J. Mele `Topological insulators in three dimensions', Phys.
Rev. Lett. 98, 106803 (2007)
[36] J. E. Moore and L. Balents `Topological invariants of timereversalinvariant band
structures', Phys. Rev. B 75, 121306 (2007)
[37] L. Fu and C. L. Kane `Topological insulators with inversion symmetry', Phys. Rev.
B 76, 045302 (2007)
[38] D. Hsieh, D. Qian, L. Wray, Y. Xia, Y. S. Hor, R. J. Cava, and M. Z. Hasan `A
topological Dirac insulator in a quantum spin hall phase', Nature 452, 970 (2008)
[39] H. Zhang, C.X. Liu, X.L. Qi, X. Dai, Z. Fang, and S.C. Zhang `Topological
insulators in Bi2Se3, Bi2Te3 and Sb2Te3 with a single Dirac cone on the surface',
Nat. Phys. 5, 438 (2009)
[40] Y. Xia, D. Qian, D. Hsieh, L. Wray, A. Pal, H. Lin, A. Bansil, D. Grauer, Y. S. Hor,
R. J. Cava, and M. Z. Hasan `Observation of a largegap topologicalinsulator class
with a single Dirac cone on the surface', Nat. Phys. 5, 398 (2009)
[41] Y. L. Chen, J. G. Analytis, J.H. Chu, Z. K. Liu, S.K. Mo, X. L. Qi, H. J. Zhang,
D. H. Lu, X. Dai, Z. Fang, S. C. Zhang, I. R. Fisher, Z. Hussain, and Z.X. Shen `Ex
perimental realization of a threedimensional topological insulator, Bi2Te3', Science
325, 178 (2009)
[42] M. König, H. Buhmann, L. W. Molenkamp, T. Hughes, C.X. Liu, X.L. Qi, and
S.C. Zhang `The quantum spin hall eect: Theory and experiment', J. Phys. Soc.
Jpn. 77, 031007 (2008)
[43] C. L. Kane `Condensed matter: An insulator with a twist', Nat. Phys. 4, 348 (2008)
[44] S.C. Zhang `Topological states of quantum matter', Physics 1, 6 (2008)
84
Bibliography
[45] J. E. Moore `The birth of topological insulators', Nature 464, 194 (2010)
[46] M. Z. Hasan and C. L. Kane `Colloquium', Rev. Mod. Phys. 82, 3045 (2010)
[47] M. Franz `Topological insulators: Starting a new family', Nat. Mater. 9, 536 (2010)
[48] X.L. Qi and S.C. Zhang `Topological insulators and superconductors', Rev. Mod.
Phys. 83, 1057 (2011)
[49] Y. L. Chen, Z. K. Liu, J. G. Analytis, J.H. Chu, H. J. Zhang, B. H. Yan, S.K.
Mo, R. G. Moore, D. H. Lu, I. R. Fisher, S. C. Zhang, Z. Hussain, and Z.X. Shen
`Single Dirac cone topological surface state and unusual thermoelectric property of
compounds from a new topological insulator family', Phys. Rev. Lett. 105, 266401
(2010)
[50] T. Sato, K. Segawa, H. Guo, K. Sugawara, S. Souma, T. Takahashi, and Y. Ando `Di
rect evidence for the Diraccone topological surface states in the ternary chalcogenide
TlBiSe2', Phys. Rev. Lett. 105, 136802 (2010)
[51] Y. S. Hor, A. Richardella, P. Roushan, Y. Xia, J. G. Checkelsky, A. Yazdani, M. Z.
Hasan, N. P. Ong, and R. J. Cava `ptype Bi2Se3 for topological insulator and low
temperature thermoelectric applications', Phys. Rev. B 79, 195208 (2009)
[52] J. G. Analytis, R. D. McDonald, S. C. Riggs, J.H. Chu, G. S. Boebinger, and I. R.
Fisher `Twodimensional surface state in the quantum limit of a topological insulator',
Nat. Phys. 6, 960 (2010)
[53] D. Kong, Y. Chen, J. J. Cha, Q. Zhang, J. G. Analytis, K. Lai, Z. Liu, S. S. Hong,
K. J. Koski, S.K. Mo, Z. Hussain, I. R. Fisher, Z.X. Shen, and Y. Cui `Ambipolar
eld eect in the ternary topological insulator (BixSb1−x)2Te3 by composition tuning',
Nat. Nano. 6, 705 (2011)
[54] J. Zhang, C.Z. Chang, Z. Zhang, J. Wen, X. Feng, K. Li, M. Liu, K. He,
L. Wang, X. Chen, Q.K. Xue, X. Ma, and Y. Wang `Band structure engineering in
(Bi1−xSbx)2Te3 ternary topological insulators', Nat. Commun. 2, 574 (2011)
[55] T. Arakane, T. Sato, S. Souma, K. Kosaka, K. Nakayama, M. Komatsu, T. Takahashi,
Z. Ren, K. Segawa, and Y. Ando `Tunable Dirac cone in the topological insulator
Bi2−xSbxTe3−ySey', Nat. Commun. 3, 636 (2012)
85
Bibliography
[56] J. G. Checkelsky, Y. S. Hor, R. J. Cava, and N. P. Ong `Bulk band gap and sur
face state conduction observed in voltagetuned crystals of the topological insulator
Bi2Se3', Phys. Rev. Lett. 106, 196801 (2011)
[57] H. Peng, K. Lai, D. Kong, S. Meister, Y. Chen, X.L. Qi, S.C. Zhang, Z.X. Shen,
and Y. Cui `Aharonovbohm interference in topological insulator nanoribbons', Nat.
Mater. 9, 225 (2010)
[58] X. Chen, X.C. Ma, K. He, J.F. Jia, and Q.K. Xue `Molecular beam epitaxial
growth of topological insulators', Advanced Materials 23, 1162 (2011)
[59] S. Das Sarma and Q. Li `Manybody eects and possible superconductivity in the
twodimensional metallic surface states of threedimensional topological insulators',
Phys. Rev. B 88, 081404 (2013)
[60] S. A. Wolf, D. D. Awschalom, R. A. Buhrman, J. M. Daughton, S. von MolnÃ½r,
M. L. Roukes, A. Y. Chtchelkanova, and D. M. Treger `Spintronics: A spinbased
electronics vision for the future', Science 294, 1488 (2001)
[61] D. Hsieh, Y. Xia, L. Wray, D. Qian, A. Pal, J. H. Dil, J. Osterwalder, F. Meier,
G. Bihlmayer, C. L. Kane, Y. S. Hor, R. J. Cava, and M. Z. Hasan `Observation of
unconventional quantum spin textures in topological insulators', Science 323, 919
(2009)
[62] J. Linder, Y. Tanaka, T. Yokoyama, A. Sudbø, and N. Nagaosa `Unconventional
superconductivity on a topological insulator', Phys. Rev. Lett. 104, 067001 (2010)
[63] C. R. Ast, G. Wittich, P. Wahl, R. Vogelgesang, D. Pacilé, M. C. Falub, L. Mores
chini, M. Papagno, M. Grioni, and K. Kern `Local detection of spinorbit splitting
by scanning tunneling spectroscopy', Phys. Rev. B 75, 201401 (2007)
[64] C. R. Ast, J. Henk, A. Ernst, L. Moreschini, M. C. Falub, D. Pacilé, P. Bruno,
K. Kern, and M. Grioni `Giant spin splitting through surface alloying', Phys. Rev.
Lett. 98, 186807 (2007)
[65] L. Moreschini, A. Bendounan, I. Gierz, C. R. Ast, H. Mirhosseini, H. Höchst, K. Kern,
J. Henk, A. Ernst, S. Ostanin, F. Reinert, and M. Grioni `Assessing the atomic
contribution to the rashba spinorbit splitting in surface alloys: Sb/Ag(111)', Phys.
Rev. B 79, 075424 (2009)
86
Bibliography
[66] G. Bihlmayer, S. Blügel, and E. V. Chulkov `Enhanced Rashba spinorbit splitting
in Bi/Ag(111) and Pb/Ag(111) surface alloys from rst principles', Phys. Rev. B
75, 195414 (2007)
[67] F. Meier, H. Dil, J. LoboCheca, L. Patthey, and J. Osterwalder `Quantitative vec
torial spin analysis in angleresolved photoemission: Bi/Ag(111) and Pb/Ag(111)',
Phys. Rev. B 77, 165431 (2008)
[68] J. Premper, M. Trautmann, J. Henk, and P. Bruno `Spinorbit splitting in an
anisotropic twodimensional electron gas', Phys. Rev. B 76, 073310 (2007)
[69] P. R. Wallace `The band theory of graphite', Phys. Rev. 71, 622 (1947)
[70] K. S. Novoselov, A. K. Geim, S. V. Morozov, D. Jiang, Y. Zhang, S. V. Dubonos,
I. V. Grigorieva, and A. A. Firsov `Electric eld eect in atomically thin carbon
lms', Science 306, 666 (2004)
[71] K. S. Novoselov, A. K. Geim, S. V. Morozov, D. Jiang, M. I. Katsnelson, I. V.
Grigorieva, S. V. Dubonos, and A. A. Firsov `Twodimensional gas of massless Dirac
fermions in graphene', Nature 438, 197 (2005)
[72] Y. Zhang, Y.W. Tan, H. L. Stormer, and P. Kim `Experimental observation of the
quantum hall eect and Berry's phase in graphene', Nature 438, 201 (2005)
[73] A. K. Geim and K. S. Novoselov `The rise of graphene', Nat. Mater. 6, 183 (2007)
[74] P. Sharma, J. GomezDiaz, A. Ionescu, and J. PerruisseauCarrier `Determination of
minimum conductivity of graphene from contactless microwaves measurements', In
`Nanotechnology (IEEENANO), 12th IEEE Conference on', pages 14 (2012)
[75] Y. Zhang, V. W. Brar, C. Girit, A. Zettl, and M. F. Crommie `Origin of spatial
charge inhomogeneity in graphene', Nat. Phys. 5, 722 (2009)
[76] A. K. Geim `Graphene: Status and prospects', Science 324, 1530 (2009)
[77] C. McConville, D. Woodru, and S. Kevan `The electronic structure of graphitic
overlayers on Ni(100)', Surface Science 171, (1986)
[78] A. M. Shikin, G. V. Prudnikova, V. K. Adamchuk, F. Moresco, and K.H. Rieder
`Surface intercalation of gold underneath a graphite monolayer on Ni(111) studied by
87
Bibliography
angleresolved photoemission and highresolution electronenergyloss spectroscopy',
Phys. Rev. B 62, 13202 (2000)
[79] A. Varykhalov, J. SánchezBarriga, A. M. Shikin, C. Biswas, E. Vescovo, A. Rybkin,
D. Marchenko, and O. Rader `Electronic and magnetic properties of quasifreestanding
graphene on Ni', Phys. Rev. Lett. 101, 157601 (2008)
[80] A. B. Preobrajenski, M. L. Ng, A. S. Vinogradov, and N. Mårtensson `Controlling
graphene corrugation on latticemismatched substrates', Phys. Rev. B 78, 073401
(2008)
[81] N. Kholin, E. Rut'kov, and A. Tontegode `The nature of the adsorption bond between
graphite islands and iridium surface', Surface Science 139, 155 (1984)
[82] I. Pletikosi¢, M. Kralj, P. Pervan, R. Brako, J. Coraux, A. T. N'Diaye, C. Busse,
and T. Michely `Dirac cones and minigaps for graphene on Ir(111)', Phys. Rev. Lett.
102, 056808 (2009)
[83] H. ZiPu, D. Ogletree, M. V. Hove, and G. Somorjai. `Leed theory for incommen
surate overlayers: Application to graphite on Pt(111)', Surface Science 180, 433
(1987)
[84] M. Sasaki, Y. Yamada, Y. Ogiwara, S. Yagyu, and S. Yamamoto `Moiré contrast in
the local tunneling barrier height images of monolayer graphite on Pt(111)', Phys.
Rev. B 61, 15653 (2000)
[85] A. V. Bommel, J. Crombeen, and A. V. Tooren `LEED and auger electron observa
tions of the SiC(0001) surface', Surface Science 48, 463 (1975)
[86] M. Orlita, C. Faugeras, P. Plochocka, P. Neugebauer, G. Martinez, D. K. Maude,
A.L. Barra, M. Sprinkle, C. Berger, W. A. de Heer, and M. Potemski `Approaching
the Dirac point in highmobility multilayer epitaxial graphene', Phys. Rev. Lett. 101,
267601 (2008)
[87] M. Sprinkle, D. Siegel, Y. Hu, J. Hicks, A. Tejeda, A. TalebIbrahimi, P. Le Fèvre,
F. Bertran, S. Vizzini, H. Enriquez, S. Chiang, P. Soukiassian, C. Berger, W. A.
de Heer, A. Lanzara, and E. H. Conrad `First direct observation of a nearly ideal
graphene band structure', Phys. Rev. Lett. 103, 226803 (2009)
88
Bibliography
[88] F. Varchon, R. Feng, J. Hass, X. Li, B. N. Nguyen, C. Naud, P. Mallet, J.Y. Veuillen,
C. Berger, E. H. Conrad, and L. Magaud `Electronic structure of epitaxial graphene
layers on SiC: Eect of the substrate', Phys. Rev. Lett. 99, 126805 (2007)
[89] T. Seyller, A. Bostwick, K. V. Emtsev, K. Horn, L. Ley, J. L. McChesney, T. Ohta,
J. D. Riley, E. Rotenberg, and F. Speck `Epitaxial graphene: a new material', Physica
status solidi (b) 245, 1436 (2008)
[90] C. Berger, Z. Song, T. Li, X. Li, A. Y. Ogbazghi, R. Feng, Z. Dai, A. N. Marchenkov,
E. H. Conrad, P. N. First, and W. A. de Heer `Ultrathin epitaxial graphite: 2D
electron gas properties and a route toward graphenebased nanoelectronics', J. Phys.
Chem. B 108, 19912 (2004)
[91] K. V. Emtsev, F. Speck, T. Seyller, L. Ley, and J. D. Riley `Interaction, growth, and
ordering of epitaxial graphene on SiC0001 surfaces: A comparative photoelectron
spectroscopy study', Phys. Rev. B 77, 155303 (2008)
[92] J. Jobst, D. Waldmann, F. Speck, R. Hirner, D. K. Maude, T. Seyller, and H. B.
Weber `Quantum oscillations and quantum hall eect in epitaxial graphene', Phys.
Rev. B 81, 195434 (2010)
[93] F. Owman, C. Hallin, P. Mårtensson, and E. Janzén `Removal of polishinginduced
damage from 6HSiC(0001) substrates by hydrogen etching', Journal of Crystal
Growth 167, 391 (1996)
[94] V. Ramachandran, M. Brady, A. Smith, R. Feenstra, and D. Greve `Preparation
of atomically at surfaces on silicon carbide using hydrogen etching', Journal of
Electronic Materials 27, 308 (1998)
[95] K. V. Emtsev, A. Bostwick, K. Horn, J. Jobst, G. L. Kellogg, L. Ley, J. L. McChesney,
T. Ohta, S. A. Reshanov, J. Rohrl, E. Rotenberg, A. K. Schmid, D. Waldmann, H. B.
Weber, and T. Seyller `Towards wafersize graphene layers by atmospheric pressure
graphitization of silicon carbide', Nat. Mater. 8, 203 (2009)
[96] C. Riedl, C. Coletti, and U. Starke `Structural and electronic properties of epitaxial
graphene on SiC(0 0 0 1): a review of growth, characterization, transfer doping and
hydrogen intercalation', Journal of Physics D: Applied Physics 43, 374009 (2010)
89
Bibliography
[97] C. Riedl, C. Coletti, T. Iwasaki, A. A. Zakharov, and U. Starke `Quasifreestanding
epitaxial graphene on SiC obtained by hydrogen intercalation', Phys. Rev. Lett. 103,
246804 (2009)
[98] A. Bostwick, T. Ohta, J. L. McChesney, K. V. Emtsev, T. Seyller, K. Horn, and
E. Rotenberg `Symmetry breaking in few layer graphene lms', New Journal of
Physics 9, 385 (2007)
[99] C. Riedl, U. Starke, J. Bernhardt, M. Franke, and K. Heinz `Structural properties
of the grapheneSiC(0001) interface as a key for the preparation of homogeneous
largeterrace graphene surfaces', Phys. Rev. B 76, 245406 (2007)
[100] P. Mallet, F. Varchon, C. Naud, L. Magaud, C. Berger, and J.Y. Veuillen `Elec
tron states of mono and bilayer graphene on SiC probed by scanningtunneling
microscopy', Phys. Rev. B 76, 041403 (2007)
[101] A. Bostwick, T. Ohta, T. Seyller, K. Horn, and E. Rotenberg `Quasiparticle dynamics
in graphene', Nat. Phys. 3, 36 (2007)
[102] T. Ohta, A. Bostwick, T. Seyller, K. Horn, and E. Rotenberg `Controlling the
electronic structure of bilayer graphene', Science 313, 951 (2006)
[103] S. Y. Zhou, G.H. Gweon, A. V. Fedorov, P. N. First, W. A. de Heer, D.H. Lee,
F. Guinea, A. H. Castro Neto, and A. Lanzara `Substrateinduced bandgap opening
in epitaxial graphene', Nat. Mater. 6, 770 (2007)
[104] J. A. Robinson, M. Wetherington, J. L. Tedesco, P. M. Campbell, X. Weng, J. Stitt,
M. A. Fanton, E. Frantz, D. Snyder, B. L. VanMil, G. G. Jernigan, R. L. Myers
Ward, C. R. Eddy, and D. K. Gaskill `Correlating Raman spectral signatures with
carrier mobility in epitaxial graphene: A guide to achieving high mobility on the
wafer scale', Nano Letters 9, 2873 (2009)
[105] H. Hertz `Über einen Einuss des ultravioletten Lichtes auf die electrische Entladung',
Annalen der Physik 267, 983 (1887)
[106] A. Einstein `Über einen die Erzeugung und Verwandlung des Lichtes betreenden
heuristischen Gesichtspunkt', Annalen der Physik 322, 132 (1905)
[107] S. Hüfner Photoelectron Spectroscopy  Principles and Applications, Springer Berlin
(2003)
90
Bibliography
[108] M. P. Seah and W. A. Dench `Quantitative electron spectroscopy of surfaces: A
standard data base for electron inelastic mean free paths in solids', Surface and
Interface Analysis 1, 2 (1979)
[109] C. N. Berglund and W. E. Spicer `Photoemission studies of copper and silver: The
ory', Phys. Rev. 136, A1030 (1964)
[110] F. Reinert `Spinorbit interaction in the photoemission spectra of noble metal surface
states'. Journal of Physics: Condensed Matter 15, S693 (2003)
[111] P. B. Allen `Electronphonon eects in the infrared properties of metals', Phys. Rev.
B 3, 305 (1971)
[112] S. Tougaard `Quantitative analysis of the inelastic background in surface electron
spectroscopy', Surface and Interface Analysis 11, 453 (1988)
[113] Moulder Handbook of Xray Photoelectron Spectroscopy, Physical Electronics (Inc.
Minnesota USA) (1995)
[114] D. Hsieh, Y. Xia, D. Qian, L. Wray, J. H. Dil, F. Meier, J. Osterwalder, L. Patthey,
J. G. Checkelsky, N. P. Ong, A. V. Fedorov, H. Lin, A. Bansil, D. Grauer, Y. S. Hor,
R. J. Cava, and M. Z. Hasan `A tunable topological insulator in the spin helical
Dirac transport regime', Nature 460, 1101 (2009)
[115] B. Sacepe, J. B. Oostinga, J. Li, A. Ubaldini, N. J. Couto, E. Giannini, and A. F.
Morpurgo `Gatetuned normal and superconducting transport at the surface of a
topological insulator', Nat. Commun. 2, 575 (2011)
[116] F. Xiu, L. He, Y. Wang, L. Cheng, L.T. Chang, M. Lang, G. Huang, X. Kou,
Y. Zhou, X. Jiang, Z. Chen, J. Zou, A. Shailos, and K. L. Wang `Manipulating
surface states in topological insulator nanoribbons', Nat. Nano. 6, 216 (2011)
[117] J. Chen, H. J. Qin, F. Yang, J. Liu, T. Guan, F. M. Qu, G. H. Zhang, J. R. Shi, X. C.
Xie, C. L. Yang, K. H. Wu, Y. Q. Li, and L. Lu `Gatevoltage control of chemical
potential and weak antilocalization in Bi2Se3', Phys. Rev. Lett. 105, 176602 (2010)
[118] D. Kong, W. Dang, J. J. Cha, H. Li, S. Meister, H. Peng, Z. Liu, and Y. Cui `Few
layer nanoplates of Bi2Se3 and Bi2Te3 with highly tunable chemical potential', Nano
Letters 10, 2245 (2010)
91
Bibliography
[119] Z. Ren, A. A. Taskin, S. Sasaki, K. Segawa, and Y. Ando `Large bulk resistivity and
surface quantum oscillations in the topological insulator Bi2Te2Se', Phys. Rev. B 82,
241306 (2010)
[120] J. Wang, A. M. DaSilva, C.Z. Chang, K. He, J. K. Jain, N. Samarth, X.C. Ma, Q.
K. Xue, and M. H. W. Chan `Evidence for electronelectron interaction in topological
insulator thin lms', Phys. Rev. B 83, 245438 (2011)
[121] Y. Takagaki, B. Jenichen, U. Jahn, M. Ramsteiner, and K.J. Friedland `Weak
antilocalization and electronelectron interaction eects in Cudoped Bi2Se3 lms',
Phys. Rev. B 85, 115314 (2012)
[122] H. K. Pal, V. I. Yudson, and D. L. Maslov `Eect of electronelectron interaction on
surface transport in the Bi2Te3 family of threedimensional topological insulators',
Phys. Rev. B 85, 085439 (2012)
[123] P. M. Ostrovsky, I. V. Gornyi, and A. D. Mirlin `Interactioninduced criticality in
Z2 topological insulators', Phys. Rev. Lett. 105, 036803 (2010)
[124] L. A. Wray, S.Y. Xu, Y. Xia, D. Hsieh, A. V. Fedorov, Y. S. Hor, R. J. Cava,
A. Bansil, H. Lin, and M. Z. Hasan `A topological insulator surface under strong
coulomb, magnetic and disorder perturbations', Nat. Phys. 7, 32 (2011)
[125] M. Hohenadler and F. F. Assaad `Correlation eects in twodimensional topological
insulators', Journal of Physics: Condensed Matter 25, 143201 (2013)
[126] J. Xiong, A. Petersen, D. Qu, Y. Hor, R. Cava, and N. Ong `Quantum oscillations
in a topological insulator Bi2Te2Se with large bulk resistivity', Physica E: Low
dimensional Systems and Nanostructures 44, 917 (2012)
[127] H. M. Benia, C. Lin, K. Kern, and C. R. Ast `Reactive chemical doping of the Bi2Se3
topological insulator', Phys. Rev. Lett. 107, 177602 (2011)
[128] M. Bianchi, R. C. Hatch, D. Guan, T. Planke, J. Mi, B. B. Iversen, and P. Hofmann
`The electronic structure of clean and adsorbatecovered Bi2Se3: an angleresolved
photoemission study', Semiconductor Science and Technology 27, 124001 (2012)
[129] R. C. Hatch, M. Bianchi, D. Guan, S. Bao, J. Mi, B. B. Iversen, L. Nilsson,
L. Hornekær, and P. Hofmann `Stability of the Bi2Se3(111) topological state:
Electronphonon and electrondefect scattering', Phys. Rev. B 83, 241303 (2011)
92
Bibliography
[130] M. Hengsberger, R. Frésard, D. Purdie, P. Segovia, and Y. Baer `Electronphonon
coupling in photoemission spectra', Phys. Rev. B 60, 10796 (1999)
[131] A. A. Kordyuk, S. V. Borisenko, A. Koitzsch, J. Fink, M. Knupfer, and H. Berger
`Bare electron dispersion from experiment: Selfconsistent selfenergy analysis of
photoemission data', Phys. Rev. B 71, 214513 (2005)
[132] K. Yang, W. Setyawan, S. Wang, M. Buongiorno Nardelli, and S. Curtarolo `A search
model for topological insulators with highthroughput robustness descriptors', Nat.
Mater. 11, 614 (2012)
[133] Z. Zhu, Y. Cheng, and U. Schwingenschlögl `Topological phase diagrams of bulk and
monolayer TiS2−xTex', Phys. Rev. Lett. 110, 077202 (2013)
[134] S.Y. Xu `Discovery of several large families of topological insulator classes
with backscatteringsuppressed spinpolarized singleDiraccone on the surface'
arXiv:1007.5111v1 (2010)
[135] J. Wilson and A. Yoe `The transition metal dichalcogenides discussion and inter
pretation of the observed optical, electrical and structural properties', Advances in
Physics 18, 193 (1969)
[136] R. Friend and A. Yoe `Electronic properties of intercalation complexes of the tran
sition metal dichalcogenides', Advances in Physics 36, 1 (1987)
[137] A. H. Castro Neto `Charge density wave, superconductivity, and anomalous metallic
behavior in 2D transition metal dichalcogenides', Phys. Rev. Lett. 86, 4382 (2001)
[138] Y. Arnaud and M. Chevreton `Etude comparative des composÃ c©s TiX2 (X = S,
Se, Te). structures de TiTe2 et TiSeTe', Journal of Solid State Chemistry 39, 230
(1981)
[139] A. Shkvarin, Y. Yarmoshenko, N. Skorikov, M. Yablonskikh, A. Merentsov, E. Shk
varina, and A. Titov `Electronic structure of titanium dichalcogenides TiX2 (X = S,
Se, Te)', Journal of Experimental and Theoretical Physics 114, 150 (2012)
[140] Y.W. Z. Hongliang Shi, Hui Pan and B. I. Yakobson `Quasiparticle band structures
and optical properties of strained monolayer MoS2 and WS2', Phys. Rev. B 87,
155304 (2013)
93
Bibliography
[141] L. Shao, G. Chen, H. Ye, Y. Wu, H. Niu, and Y. Zhu `Theoretical study on electronic
properties of MoS2 antidot lattices', Journal of Applied Physics 116, 113704 (2014)
[142] A. K. Geim and I. V. Grigorieva `Van der waals heterostructures', Nature 499, 419
(2013)
[143] D. Kong and Y. Cui `Opportunities in chemistry and materials science for topological
insulators and their nanostructures', Nat. Chem. 3, 845 (2011)
[144] M. Chhowalla, H. S. Shin, G. Eda, L.J. Li, K. P. Loh, and H. Zhang `The chemistry
of twodimensional layered transition metal dichalcogenide nanosheets', Nat. Chem.
5, 263 (2013)
[145] H. L. Zhuang and R. G. Hennig `Computational search for singlelayer transition
metal dichalcogenide photocatalysts', The Journal of Physical Chemistry C 117,
20440 (2013)
[146] D. Jariwala, V. K. Sangwan, L. J. Lauhon, T. J. Marks, and M. C. Hersam `Emerging
device applications for semiconducting twodimensional transition metal dichalco
genides', ACS Nano 8, 1102 (2014)
[147] Q. H. Wang, K. KalantarZadeh, A. Kis, J. N. Coleman, and M. S. Strano `Electronics
and optoelectronics of twodimensional transition metal dichalcogenides', Nat. Nano.
7, 699 (2012)
[148] H. Pan `Metal dichalcogenides monolayers: Novel catalysts for electrochemical hy
drogen production', Sci. Rep. 4, 5348 (2014)
[149] E. Gourmelon, O. Lignier, H. Hadouda, G. Couturier, J. Bernede, J. Tedd, J. Pouzet,
and J. Salardenne `MS2 (M= W, Mo) photosensitive thin lms for solar cells', Solar
Energy Materials and Solar Cells 46, 115 (1997)
[150] T. Cao, G. Wang, W. Han, H. Ye, C. Zhu, J. Shi, Q. Niu, P. Tan, E. Wang, B. Liu, and
J. Feng `Valleyselective circular dichroism of monolayer molybdenum disulphide',
Nat. Commun. 3, 887 (2012)
[151] K. F. Mak, K. He, J. Shan, and T. F. Heinz `Control of valley polarization in
monolayer MoS2 by optical helicity', Nat. Nano. 7, 494 (2012)
94
Bibliography
[152] W. Chen, S. Chen, D. C. Qi, X. Y. Gao, and A. T. S. Wee `Surface transfer ptype
doping of epitaxial graphene', Journal of the American Chemical Society 129, 10418
(2007)
[153] C. Coletti, C. Riedl, D. S. Lee, B. Krauss, L. Patthey, K. von Klitzing, J. H. Smet,
and U. Starke `Charge neutrality and bandgap tuning of epitaxial graphene on SiC
by molecular doping', Phys. Rev. B 81, 235401 (2010)
[154] I. Gierz, C. Riedl, U. Starke, C. R. Ast, and K. Kern `Atomic hole doping of
graphene', Nano Letters 8, 4603 (2008)
[155] K. Pi, K. M. McCreary, W. Bao, W. Han, Y. F. Chiang, Y. Li, S.W. Tsai, C. N.
Lau, and R. K. Kawakami `Electronic doping and scattering by transition metals on
graphene', Phys. Rev. B 80, 075406 (2009)
[156] T. O. Wehling, K. S. Novoselov, S. V. Morozov, E. E. Vdovin, M. I. Katsnelson,
A. K. Geim, and A. I. Lichtenstein `Molecular doping of graphene', Nano Letters 8,
173 (2008)
[157] D. A. Siegel, C.H. Park, C. Hwang, J. Deslippe, A. V. Fedorov, S. G. Louie, and
A. Lanzara `Manybody interactions in quasifreestanding graphene', Proceedings of
the National Academy of Sciences 108, 11365 (2011)
[158] J. L. McChesney, A. Bostwick, T. Ohta, T. Seyller, K. Horn, J. González, and
E. Rotenberg `Extended van Hove singularity and superconducting instability in
doped graphene', Phys. Rev. Lett. 104, 136803 (2010)
[159] A. Bostwick, J. L. McChesney, K. V. Emtsev, T. Seyller, K. Horn, S. D. Kevan, and
E. Rotenberg `Quasiparticle transformation during a metalinsulator transition in
graphene', Phys. Rev. Lett. 103, 056404 (2009)
[160] G. Schubert and H. Fehske `Metaltoinsulator transition and electronhole puddle
formation in disordered graphene nanoribbons', Phys. Rev. Lett. 108, 066402 (2012)
[161] G. Profeta, M. Calandra, and F. Mauri `Phononmediated superconductivity in
graphene by lithium deposition', Nat. Phys. 8, 131 (2012)
[162] C. Weeks, J. Hu, J. Alicea, M. Franz, and R. Wu `Engineering a robust quantum
spin hall state in graphene via adatom deposition', Phys. Rev. X 1, 021001 (2011)
95
Bibliography
[163] N. M. R. Peres `The transport properties of graphene: An introduction', Rev. Mod.
Phys. 82, 2673 (2010)
[164] H. Medina, Y.C. Lin, D. Obergfell, and P.W. Chiu `Tuning of charge densities in
graphene by molecule doping', Advanced Functional Materials 21, 2687 (2011)
[165] F. Schedin, A. K. Geim, S. V. Morozov, E. W. Hill, P. Blake, M. I. Katsnelson, and
K. S. Novoselov `Detection of individual gas molecules adsorbed on graphene', Nat.
Mater. 6, 652 (2007)
[166] D. A. Siegel, W. Regan, A. V. Fedorov, A. Zettl, and A. Lanzara `Charge carrier
screening in single layer graphene', Phys. Rev. Lett. 110, 146802 (2013)
[167] T. Wehling, M. Katsnelson, and A. Lichtenstein `Adsorbates on graphene: Impurity
states and electron scattering', Chem. Phys. Lett. 476, 125 (2009)
[168] K. Nakada and A. Ishii `Migration of adatom adsorption on graphene using DFT
calculation', Solid State Communications 151, 13 (2011)
[169] J.H. Chen, C. Jang, S. Adam, M. S. Fuhrer, E. D. Williams, and M. Ishigami
`Chargedimpurity scattering in graphene', Nat. Phys. 4, 377 (2008)
[170] F. de Juan, E. H. Hwang, and M. A. H. Vozmediano `Spectral and optical properties
of doped graphene with charged impurities in the selfconsistent born approximation',
Phys. Rev. B 82, 245418 (2010)
[171] E. H. Hwang and S. Das Sarma `Singleparticle relaxation time versus transport
scattering time in a twodimensional graphene layer', Phys. Rev. B 77, 195412
(2008)
[172] A. L. Walter, A. Bostwick, K.J. Jeon, F. Speck, M. Ostler, T. Seyller, L. Moreschini,
Y. J. Chang, M. Polini, R. Asgari, A. H. MacDonald, K. Horn, and E. Rotenberg
`Eective screening and the plasmaron bands in graphene', Phys. Rev. B 84, 085410
(2011)
[173] T. Horiguchi `Lattice green's functions for the triangular and honeycomb lattices',
J. Math. Phys. 13, 1411 (1972)
96
Bibliography
[174] J. Lischner, D. VigilFowler, and S. G. Louie `Physical origin of satellites in photoe
mission of doped graphene: An ab initio GW plus cumulant study', Phys. Rev. Lett.
110, 146801 (2013)
[175] C. Hwang, D. A. Siegel, S.K. Mo, W. Regan, A. Ismach, Y. Zhang, A. Zettl, and
A. Lanzara `Fermi velocity engineering in graphene by substrate modication', Sci.
Rep. 2, 590 (2012)
[176] J. P. Robinson, H. Schomerus, L. Oroszlány, and V. I. Fal'ko `Adsorbatelimited
conductivity of graphene', Phys. Rev. Lett. 101, 196803 (2008)
[177] P. A. Wol `Localized moments in metals', Phys. Rev. 124, 1030 (1961)
[178] A. M. Clogston, B. T. Matthias, M. Peter, H. J. Williams, E. Corenzwit, and R. C.
Sherwood `Local magnetic moment associated with an iron atom dissolved in various
transition metal alloys', Phys. Rev. 125, 541 (1962)
[179] B. Velický, S. Kirkpatrick, and H. Ehrenreich `Singlesite approximations in the
electronic theory of simple binary alloys', Phys. Rev. 175, 747 (1968)
[180] J. Zhenzhao `Absence of a transport signature of spinorbit coupling in graphene
with indium adatoms', arXiv:1409.8090 (2014)
[181] Y.W. Tan, Y. Zhang, K. Bolotin, Y. Zhao, S. Adam, E. H. Hwang, S. Das Sarma,
H. L. Stormer, and P. Kim `Measurement of scattering rate and minimum conduc
tivity in graphene', Phys. Rev. Lett. 99, 246803 (2007)
[182] S. Das Sarma, S. Adam, E. H. Hwang, and E. Rossi `Electronic transport in two
dimensional graphene', Rev. Mod. Phys. 83, 407 (2011)
[183] M. I. Katsnelson Graphene: Carbon in Two Dimensions, Cambridge University
Press (2012)
[184] E. Hwang, S. Adam, and S. Das Sarma `Carrier transport in twodimensional
graphene layers', Phys. Rev. Lett. 98, 186806 (2007)
[185] K. Nomura and MacDonald `Quantum transport of massless Dirac fermions', Phys.
Rev. Lett. 98, 076602 (2007)
97
Bibliography
[186] Y. H. Wang, D. Hsieh, D. Pilon, L. Fu, D. R. Gardner, Y. S. Lee, and N. Gedik.
`Observation of a warped helical spin texture in Bi2Se3 from circular dichroism angle
resolved photoemission spectroscopy', Phys. Rev. Lett. 107, 207602 (2011)
[187] G. Bian, L. Zhang, Y. Liu, T. Miller, and T.C. Chiang `Illuminating the surface spin
texture of the giantRashba quantumwell system Bi/Ag(111) by circularly polarized
photoemission', Phys. Rev. Lett. 108, 186403 (2012)
[188] Y. Wang and N. Gedik `Circular dichroism in angleresolved photoemission spec
troscopy of topological insulators', physica status solidi (RRL) Rapid Research Let
ters 7, 64 (2013)
[189] J. SánchezBarriga, A. Varykhalov, J. Braun, S.Y. Xu, N. Alidoust, O. Kornilov,
J. Minár, K. Hummer, G. Springholz, G. Bauer, R. Schumann, L. V. Yashina,
H. Ebert, M. Z. Hasan, and O. Rader `Photoemission of Bi2Se3 with circularly
polarized light: Probe of spin polarization or means for spin manipulation?', Phys.
Rev. X 4, 011046 (2014)
[190] W. Jung, Y. Kim, B. Kim, Y. Koh, C. Kim, M. Matsunami, S.i. Kimura, M. Arita,
K. Shimada, J. H. Han, J. Kim, B. Cho, and C. Kim `Warping eects in the band
and angularmomentum structures of the topological insulator Bi2Te3', Phys. Rev.
B 84, 245435 (2011)
[191] S. R. Park, J. Han, C. Kim, Y. Y. Koh, C. Kim, H. Lee, H. J. Choi, J. H. Han, K. D.
Lee, N. J. Hur, M. Arita, K. Shimada, H. Namatame, and M. Taniguchi `Chiral
orbitalangular momentum in the surface states of Bi2Se3', Phys. Rev. Lett. 108,
046805 (2012)
[192] H. Mirhosseini and J. Henk `Spin texture and circular dichroism in photoelectron
spectroscopy from the topological insulator Bi2Te3: Firstprinciples photoemission
calculations', Phys. Rev. Lett. 109, 036803 (2012)
[193] G. Schönhense `Circular dichroism and spin polarization in photoemission from
adsorbates and nonmagnetic solids', Physica Scripta 1990, 255 (1990)
[194] I. Gierz, M. Lindroos, H. Höchst, C. R. Ast, and K. Kern `Graphene sublattice sym
metry and isospin determined by circular dichroism in angleresolved photoemission
spectroscopy', Nano Letters 12, 3900 (2012)
98
Bibliography
[195] M. R. Scholz, J. SánchezBarriga, J. Braun, D. Marchenko, A. Varykhalov, M. Lin
droos, Y. J. Wang, H. Lin, A. Bansil, J. Minár, H. Ebert, A. Volykhov, L. V. Yashina,
and O. Rader `Reversal of the circular dichroism in angleresolved photoemission from
Bi2Te3', Phys. Rev. Lett. 110, 216801 (2013)
[196] J.H. Park, C. H. Kim, J.W. Rhim, and J. H. Han `Orbital rashba eect and its
detection by circular dichroism angleresolved photoemission spectroscopy', Phys.
Rev. B 85, 195401 (2012)
[197] V. Arpiainen, V. Zalobotnyy, A. A. Kordyuk, S. V. Borisenko, and M. Lindroos
`Angular dependence of circular dichroism in Pbdoped and pristine', Phys. Rev. B
77, 024520 (2008)
[198] B. Kim, C. H. Kim, P. Kim, W. Jung, Y. Kim, Y. Koh, M. Arita, K. Shimada,
H. Namatame, M. Taniguchi, J. Yu, and C. Kim `Spin and orbital angular momentum
structure of Cu(111) and Au(111) surface states', Phys. Rev. B 85, 195402 (2012)
[199] C. Jozwiak, C.H. Park, K. Gotlieb, C. Hwang, D.H. Lee, S. G. Louie, J. D. Den
linger, C. R. Rotundu, R. J. Birgeneau, Z. Hussain, and A. Lanzara `Photoelectron
spinipping and texture manipulation in a topological insulator', Nat. Phys. 9, 293
(2013)
[200] D.H. Lee `Surface states of topological insulators: The Dirac fermion in curved
twodimensional spaces', Phys. Rev. Lett. 103, 196804 (2009)
[201] H.Z. Lu, J. Shi, and S.Q. Shen `Competition between weak localization and antilo
calization in topological surface states', Phys. Rev. Lett. 107, 076801 (2011)
[202] A. P. Schnyder, S. Ryu, A. Furusaki, and A. W. W. Ludwig `Classication of topo
logical insulators and superconductors in three spatial dimensions', Phys. Rev. B 78,
195125 (2008)
[203] M. Polini, R. Asgari, G. Borghi, Y. Barlas, T. PeregBarnea, and A. H. MacDonald
`Plasmons and the spectral function of graphene', Phys. Rev. B 77, 081411 (2008)
[204] S. R. Park, W. S. Jung, C. Kim, D. J. Song, C. Kim, S. Kimura, K. D. Lee, and
N. Hur `Quasiparticle scattering and the protected nature of the topological states
in a parent topological insulator Bi2Se3', Phys. Rev. B 81, 041405 (2010)
99
Bibliography
[205] W. Y. Liu MinHao `Electron interaction and localization in ultrathin topological
insulator lms', Science China Physics, Mechanics and Astronomy 55, 2213 (2012)
[206] H.C. Liu, H.Z. Lu, H.T. He, B. Li, S.G. Liu, Q. L. He, G. Wang, I. K. Sou, S.Q.
Shen, and J. Wang `Tunable interactioninduced localization of surface electrons in
antidot nanostructured Bi2Te3 thin lms', ACS Nano 8, 9616 (2014)
[207] C. Nayak, S. H. Simon, A. Stern, M. Freedman, and S. Das Sarma `Nonabelian
anyons and topological quantum computation', Rev. Mod. Phys. 80, 1083 (2008)
[208] S. Raghu, S. B. Chung, X.L. Qi, and S.C. Zhang `Collective modes of a helical
liquid', Phys. Rev. Lett. 104, 116401 (2010)
[209] J. W. McIver and D. Hsieh and H. Steinberg and P. JarilloHerrero and N. Gedik
`Control over topological insulator photocurrents with light polarization', Nat. Nano.
7, 96 (2012)
[210] C.H. Park and S. G. Louie. `Spin polarization of photoelectrons from topological
insulators', Phys. Rev. Lett. 109, 097601 (2012)
[211] C. R. Ast, D. Pacilé, L. Moreschini, M. C. Falub, M. Papagno, K. Kern, M. Grioni,
J. Henk, A. Ernst, S. Ostanin, and P. Bruno `Spinorbit split twodimensional electron
gas with tunable Rashba and Fermi energy' Phys. Rev. B 77, 081407 (2008)
[212] R. Balog, B. Jorgensen, L. Nilsson, M. Andersen, E. Rienks, M. Bianchi, M. Fanetti,
E. Laegsgaard, A. Baraldi, S. Lizzit, Z. Sljivancanin, F. Besenbacher, B. Hammer,
T. G. Pedersen, P. Hofmann, and L. Hornekaer `Bandgap opening in graphene
induced by patterned hydrogen adsorption', Nat. Mater. 9, 315 (2010)
[213] Y.C. Chen, D. G. de Oteyza, Z. Pedramrazi, C. Chen, F. R. Fischer, and M. F.
Crommie `Tuning the band gap of graphene nanoribbons synthesized from molecular
precursors', ACS Nano 7, 6123 (2013)
[214] C. R. Woods, L. Britnell, A. Eckmann, R. S. Ma, J. C. Lu, H. M. Guo, X. Lin,
G. L. Yu, Y. Cao, R. V. Gorbachev, A. V. Kretinin, J. Park, L. A. Ponomarenko,
M. I. Katsnelson, Y. N. Gornostyrev, K. Watanabe, T. Taniguchi, C. Casiraghi, H.J.
Gao, A. K. Geim, and K. S. Novoselov `Commensurateincommensurate transition
in graphene on hexagonal boron nitride', Nat. Phys. 10, 451 (2014)
100
Bibliography
[215] H. Vita, S. Bottcher, K. Horn, E. N. Voloshina, R. E. Ovcharenko, T. Kampen,
A. Thissen, and Y. S. Dedkov `Understanding the origin of band gap formation in
graphene on metals: graphene on Cu/Ir(111)', Sci. Rep. 4, 5704 (2014)
[216] J. Hu, J. Alicea, R. Wu, and M. Franz `Giant topological insulator gap in graphene
with 5d adatoms', Phys. Rev. Lett. 109, 266801 (2012)
[217] M. Zhao, W. Dong, and A. Wang `Twodimensional carbon topological insulators
superior to graphene', Sci. Rep. 3, 3532 (2013)
[218] H. B. Heersche, P. JarilloHerrero, J. B. Oostinga, L. M. K. Vandersypen, and A. F.
Morpurgo `Bipolar supercurrent in graphene', Nature 446, 56 (2007)
[219] C. OjedaAristizabal, M. Ferrier, S. Guéron, and H. Bouchiat `Tuning the proximity
eect in a superconductorgraphenesuperconductor junction', Phys. Rev. B 79,
165436 (2009)
[220] D. Jeong, J.H. Choi, G.H. Lee, S. Jo, Y.J. Doh, and H.J. Lee `Observation of
supercurrent in PbIngraphenePbIn josephson junction', Phys. Rev. B 83, 094503
(2011)
101
Bibliography
102
Curriculum Vitae
Name
Name Carola StraÿerDate of Birth March 11, 1987Place of Birth Lauingen an der Donau, GermanyNationality German
School Education
19931997 Volksschule Wittislingen, Germany19972006 St. Bonaventura Gymnasium in Dillingen an der Donau, Germany
University Education
20062011 Studies of FOKUS Physics at the JuliusMaximiliansUniversitätWürzburg, Germany
2009 Bachelor of Science2011 Master of Science with Honors
Professional Experience
20092011 Master thesis 'Lowdimensional electron systems on semiconducting and metallic substrates' in the Group of Prof. Klaus Kern atthe Max Planck Institute for Solid State Research in Stuttgart,Germany
20112015 PhD Student in the Group of Prof. Klaus Kern at the Max PlanckInstitute for Solid State Research in Stuttgart, GermanyTopic: `Investigation of interactions in twodimensional electrongases with angular resolved photoemission spectroscopy'
2012 Research project on Tl adatoms on a monolayer of epitaxialgraphene for three months at the University of British Columbiain Vancouver in the group of Prof. Andrea Damascelli
103
104
Publications
1. M. Assig, A. Koch, W. Stiepany, C. Straÿer, A. Ast, K. Kern, and C. R. Ast
'Miniature active damping stage for scanning probe applications in ultra high vac
uum'
Rev. Sci. Instrum. 83, 033701 (2012)
2. M. Morgenstern, A. Georgi, C. Straÿer, C. R. Ast, S. Becker, and M. Liebmann
'Scanning tunneling microscopy of twodimensional semiconductors: Spin properties
and disorder'
Physica E: Lowdimensional Systems and Nanostructures 44, 1795 (2012)
3. C. Straÿer, B. M. Ludbrook, G. Levy, A. J. Macdonald, S. A. Burke, T. O. Wehling,
K. Kern, A. Damascelli, and C. R. Ast
'Longrange versus shortrange scattering in doped epitaxial graphene'
(submitted)
4. B. M. Ludbrook, G. Levy, M. Zonno, M. Schneider, D. J. Dvorak, C. N. Veenstra,
S. Zhdanovich, D. Wong, P. Dosanjh, C. Straÿer, A. Stöhr, S. Forti, C. R. Ast, U.
Starke, and A. Damascelli
'Evidence for superconductivity in Lidecorated graphene'
(submitted)
5. H. M. Benia, C. Straÿer, K. Kern, and C. R. Ast
'The surface band structure of Bi1−xSbx(111)'
(submitted)
6. C. Straÿer, I. Gierz, H. M. Benia, K. Kern, and C. R. Ast
'Photonenergy dependence of circular dichroism in the measured band structure of
surface alloys'
(in preparation)
105
106
Acknowledgements Danksagungen
Zum Erfolg dieser Arbeit haben viele Leute beigetragen. Deshalb möchte ich mich be
danken bei
Prof. Klaus Kern, der mir die Möglichkeit gegeben hat als Doktorandin in seiner Abteilung
am MaxPlanckInstitut für Festkörperforschung zu arbeiten und die verschiedenen For
schungsprojekte durchzuführen. Er hat stets dafür gesorgt, dass alle notwendigen Rah
menbedingungen bestens erfüllt waren.
Dr. Christian Ast für die direkte Betreuung meiner Arbeit, die unzähligen Ratschläge
und vielen fruchtbaren Diskussionen, für seine unglaubliche Begeisterung für die Wis
senschaft und für sein oenes Ohr. Ein groÿes Dankeschön auch für die sorgfältigen Kor
rekturen und hilfreichen Anmerkungen zu dieser Arbeit.
Prof. Andrea Damascelli for the opportunity to work for three months in his ARPES
lab in Vancouver, for his scientic support and for the successful collaboration within the
scope of the MPIUBC center.
Bart Ludbrook and Giorgio Levy for introducing me to the ARPES machine at UBC,
for the friendly and pleasant working atmosphere and for their technical assistance.
Prof. Sarah Burke and her student Andrew Macdonald for the STM measurements
on Tl decorated graphene.
Dr. Ulrich Starke, Dr. Stiven Forti, Alexander Stöhr und Axel Köhler für die
vielen hochqualitativen GraphenProben und die nette und freundliche Atmosphäre bei
der Arbeit im 7B15 Labor.
Tolga Acartürk und Arthur Küster für ihre stete und schnelle Hilfe bei allen technis
chen Problemen und Fragen im Labor.
Dr. Alexander Kuhn for growing the TiTe1.5Se0.5 samples and Dr. Chandra Shekhar
for the Bi2Te2Se crystals.
107
Dr. Thomas White for painstakingly proofreading this thesis and for always making me
smile when meeting him in the 6C oor.
Dr. Isabella Gierz dafür, dass sie mich als ihre Nachfolgerin perfekt eingelernt und mir
gezeigt hat, wie man organisiert und wissenschaftlich präzise im Labor arbeitet. Danke
auch für die schöne Zeit in Stuttgart.
Dr. Hadj Benia für die ausführliche und geduldige Einweisung im Labor und die zahlrei
chen Diskussionen.
Dr. Sören Krotzky für seine unglaubliche Hilfsbereitschaft und sein oenes Ohr zu jeder
Zeit sowohl bei physikalischen oder technischen als auch privaten Angelegenheiten.
Dr. Tobias Herden für seine freundliche Unterstützung und seine korrekte und äuÿerst
zuverlässige Art. Vielen Dank für die Unmengen an selbstgebackenen Kuchen!
meinen lieben Bürokollegen Dr. Maximilian Assig, Dr. Steen Kahle, Matthias
Eltschka und Sven Aeschlimann dafür, dass wir ein so ordentliches und harmonisches
Büroteam waren.
Christian Dette, Claudius Morchutt, Dr. Eike Oliver SchäferNolte und Ben
jamin Wurster für die unvergesslichen Fahrten mit der Schnecke im Mini!
Dr. Liza HerreraDiez for passing the responsibility of being the chocolate president on
to me. I enjoyed a lot of lovely hours eating huge amounts of chocolate and I am convinced
Diana Hötger will be a wonderful successor.
Dr. Theresa Lutz, Verena Schendel, Sabine Abb, Sebastian Koslowski für die
schönen Joggingrunden um die Bärenseen und die vielen lustigen Stunden sowohl inner
halb als auch auÿerhalb des Instituts!
meiner Familie und bei Simon für die bedingungslose Unterstützung in guten wie in
schweren Zeiten.
108